International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Microbiological deterioration and degradation of synthetic polymeric
materials: recent research advances
Ji-Dong Gua; b;∗
a Laboratory of Environmental Toxicology, Department of Ecology & Biodiversity, The University of Hong Kong, Pokfulam Road,
Hong Kong SAR, People’s Republic of China
b The Swire Institute of Marine Science, The University of Hong Kong, Shek O, Cape d’Aguilar, Hong Kong SAR, People’s Republic of China
Received 11 July 2002; received in revised form 9 September 2002; accepted 21 November 2002
Biodeterioration of polymeric materials a ect a wide range of industries. Degradability of polymeric materials is a function of the struc-
tures of polymeric materials, the presence of degradative microbial population and the environmental conditions that encourage microbial
growth. Our understanding of polymer degradation has been advanced in recent years, but the subject is still inadequately addressed. This
is clearly indicated by the lack of information available on biodeterioration of polymeric materials, particularly the mechanisms involved
and the microorganisms participated. In this review, polymers are treated according to their origin and biodegradability, and grouped as
biopolymer, chemically modiÿed natural polymers and recalcitrant polymers. Selective examples are used to illustrate the mechanisms
and microorganisms involved in degradation of speciÿc polymeric materials, and detection methods used for degradation and deterioration
tests are discussed. In addition, new detection techniques and preventive measures are also presented.
? 2003 Elsevier Ltd. All rights reserved.
Keywords: Biodeterioration; Biodegradation; Biodeteriogens; Fiber-reinforced composites; Fungi; Polymers; Prevention
1. Introduction Materials including metals (Gu et al., 2000a), inorganic
minerals (Gu et al., 1996d, 1998c, 2000c) and organic poly-
All surfaces under natural and artiÿcial conditions except mers (Gu et al., 2000b) are susceptible to the formation of
for extremely clean rooms are covered ubiquitously with microbial bioÿlms under humid conditions, particularly
microorganisms. This unique characteristic of bacterial as- those in tropical and subtropical climates (Gu et al., 2000d).
sociation with surfaces was evident from the very beginning Subsequent damage of materials is a result of natural pro-
of bacterial existence and has remained part of normal liv- cesses catalyzed by microorganisms. Complete degradation
ing (Angles et al., 1993; Gu et al., 2000b,d; Marshall, 1976, of natural materials is an important part of the nutrients
1992; Wachtershauser, 1988; Woese, 1987). The process in cycling in the ecosystem (Swift et al., 1979). Bioÿlm forma-
which a complex community of microorganisms is estab- tion is a prerequisite for substantial corrosion and/or dete-
lished on a surface is known as “microfouling” or formation rioration of the underlying materials to take place (Arino et
of bioÿlm. Bioÿlms, consisting of both microorganisms and al., 1997; Gu and Mitchell, 2001; Gu et al., 2000a–d; Hou,
their extracellular polysaccharides, are highly diverse and 1999; Saiz-Jimenez, 1995, 1997; Walch, 1992).
variable in both space and time. They are common on all sur-
faces in both terrestrial and aquatic environments (Caldwell
et al., 1997; Fletcher, 1996; Ford et al., 1991; Ford, 1993; 2. Bioÿlms and fouling on materials
Geesey and White, 1990; Gehrke et al., 1998; Neu, 1996).
Bioÿlm structures are highly organized and diverse on
∗ Corresponding author. Laboratory of Environmental Toxicology, surfaces (Bitton, 1980; Bonet et al., 1993; Breznak, 1984;
Department of Ecology & Biodiversity, The University of Hong
Kong, Pokfulam Road, Hong Kong SAR, People’s Republic of China.
Caldwell et al., 1997; Costerton et al., 1978, 1994; Dalton
Tel.: +852-2299-0605; fax: +852-2517-6082. et al., 1994; Davey and O’Toole, 2000; Freeman and Lock,
E-mail address: email@example.com (J.-D. Gu). 1995; Guezennec et al., 1998; Kelley-Wintenberg and
0964-8305/03/$ - see front matter ? 2003 Elsevier Ltd. All rights reserved.
70 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Montie, 1994; Lappin-Scott et al., 1992; L’Hostis et al., organisms on substratum surfaces (Gu and Mitchell, 1995;
1997; O’Toole et al., 2000; Whitÿeld, 1988; Wimpenny Nefedov et al., 1988; Novikova and Zaloguyev, 1985;
and Colasanti, 1997; Wolfaardt et al., 1994; Zachary Solomin, 1985; Sunesson et al., 1995; Viktorov, 1994;
et al., 1980). The speciÿc architectural structures and or- Viktorov and Novikova, 1985; Viktorov and IIyin, 1992;
ganization of microorganisms on a particular surface are Viktorov et al., 1993; Zaloguyev, 1985). The thin ÿlm on
generally materials and microorganisms speciÿc, depend- fouled surfaces usually consists of microorganisms em-
ing on the surface properties (Fletcher and Loeb, 1979; bedded in an organic matrix of biopolymers, which are pro-
van Loosdrecht et al., 1987, 1990; Wiencek and Fletcher, duced by the microorganisms under natural conditions. In
1995) and the ambient environmental conditions includ- addition, microbial precipitates, minerals, and corrosion
ing externally supplied electrical current, cationic ions, products may also coexist (Beveridge et al., 1997;
ionic concentrations, solution chemistry, and hydrodynamic Konhauser et al., 1994; Liken, 1981; Lovley, 1991; Pierson
conditions (Caldwell and Lawrence, 1986; Korber et al., and Parenteau, 2000; Wilkinson and Stark, 1956; Zehnder
1989; Lawrence et al., 1987; Lewandowski et al., 1995; and Stumm, 1988). Microfouling by microorganisms can
Leyden and Basiulis, 1989; Little et al., 1986; Marshall serve as a prerequisite for the subsequent macrofouling by
et al., 1971; Martrhamuthu et al., 1995; Neu, 1996; Pendyala invertebrates such as Balanus amphitrite, Janua brasilien-
et al., 1996; Power and Marshall, 1988; Rijnaarts et al., sis, Ciona intestinalis (Gu et al., 1997c; Maki et al., 1990).
1993; Schmidt, 1997; Sneider et al., 1994; Stoodley et al., Industrial fouling is a complex phenomenon involving inter-
1997). Because virtually all surfaces may act as substrate actions between chemical, biological and physical processes
for bacterial adhesion and bioÿlm formation (Busscher et resulting in enormous economic loss. To combat fouling
al., 1990; Costerton et al., 1995; Geesey and White, 1990; and corrosion, large quantities of biocides have been used
Geesey et al., 1996; Marshall, 1980), attack of materials by to control biofouling and as a result biocide resistance is an
microorganisms can take place either directly or indirectly, emerging problem to our society.
depending on the speciÿc microorganisms, chemical and Both metal and non-metallic materials immersed in
physical properties of the materials, and their environmental aqueous environments or under high humidity conditions
conditions (Gu et al., 2000d). More speciÿcally, important are equally susceptible to biofouling and biodeteriora-
factors a ecting the rate of biodeterioration include mate- tion (Characklis, 1990; Gu and Mitchell, 1995; Gu et al.,
rial composition (Bos et al., 1999; Busscher et al., 1990; 1998b, 2000d; Jones-Meehan et al., 1994a, b; Knyazev
Gu et al., 2000b; Wiencek and Fletcher, 1995), molecular et al., 1986; Little et al., 1990; Thorp et al., 1994). Spe-
weights, atomic composition and the chemical bonds in the ciÿc examples include medical implants (Dobbins et al.,
structure, the physical and chemical characteristics of the 1989; Gu et al., 2001a–c; McLean et al., 1995; Mittelman,
surfaces (Becker et al., 1994; Caldwell et al., 1997; Callow 1996), water pipes (Rogers et al., 1994), artiÿcial coatings
and Fletcher, 1994), the indigenous micro ora, and envi- (Edwards et al., 1994; Gu et al., 1998a; Jones-Meehan et
ronmental conditions. Using microorganisms capable of de- al., 1994b; Stern and Howard, 2000; Thorp et al., 1997),
grading speciÿc organic pollutants, the bioÿlms immobilized rubber (Berekaa et al., 2000), ultrapure systems (Flemming
on material surfaces have important applications in degra- et al., 1994; Mittelman, 1995), porous media (Bouwer,
dation of toxic pollutants, wastewater treatment and bio- 1992; Cunningham et al., 1990, 1991; Mills and Powelson,
leaching (Bryers, 1990, 1994; Gu, 2001; Gu et al., 2001c; 1996; Rittman, 1993; Vandevivere, 1995; Vandevivere and
Osswald et al., 1995; Sharp et al., 1998). In contrast, bioÿlms Kirchman, 1993; Williams and Fletcher, 1996), water and
are undesirable in food processing, drinking-water distribu- wastewater treatment (Bryers and Characklis, 1990; Gillis
tion systems, petroleum transport pipeline, water-cooling and Gillis, 1996; Rethke, 1994; Tall et al., 1995), oilÿeld
systems, on submerged engineering systems and structures, (Lynch and Edyvean, 1988), space station (Gazenko et al.,
medical implant materials. On molecular level, bacterial 1990; Meshkov, 1994; Novikova et al., 1986; Pierson and
attachment on surfaces is a process controlled by chemical Mishra, 1992; Stranger-Joannesen et al., 1993; Zaloguyev,
signaling between bacteria (Davies et al., 1998; McLean 1985) and magnetic diskettes (McCain and Mirocha, 1995).
et al., 1997; Reynolds and Fink, 2001) and the speciÿc Generally, biodeterioration is the undesirable degra-
chemical molecules involved have been elucidated as dation of materials including both metals and polymers
N -(3-oxohexanoyl)-L-acylhomoserine lactones in Photo- in the presence of and by microorganisms. Damage of
bacterium ÿsheri, N -(3-hydroxybutanoyl)-L-acylhomoserine materials may result in an early and unexpected con-
in Vibrio harveyi, N -(3-oxododecanoyl)-L-acylhomo- sequence and the problem is often translated to system
serine in Pseudomonas aeruginosa, N -(3-oxooctanoyl)-L- failure and economic loss. The term biodeterioration also
acylhomoserine in Agrobacterium tumefaciens, and implicitly includes both biocorrosion and biodegradation
-butyrolactone in Streptomyces spp. (Davies et al., 1998; in this review. All three terms, corrosion, degradation
Salmond et al., 1995; You et al., 1998). and deterioration are used in this review. In the follow-
Biofouling is a process deÿned as the undesirable accu- ing sections, microbial deterioration and degradation of
mulation of microorganisms, their products and deposits polymeric materials are discussed for several groups of
including minerals and organic materials, and macro- materials.
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 71
3. Biodeterioration of polymeric materials Polymer
Microorganisms are involved in the deterioration and Depolymerases
degradation of both synthetic and natural polymers
(Gu et al., 2000b), and very little is known about the
biodegradation of synthetic polymeric materials. The reason Dimers
is probably due to the recent development and manufac- Monomers
ture of this class of materials and the relatively slow rate Aerobic Anaerobic
of degradation in natural environments. Since chemically Microbial Biomass Microbial Biomass
synthesized polymeric materials have become an impor- CO2 CH4/H2S
tant part of our human society and have more diversiÿed H2O CO2
applications than traditional metals, issues related to poly-
mer deterioration and protection will receive increasingly
Fig. 1. Schematic diagram of polymer degradation under aerobic and
attention in the time to come. anaerobic conditions.
Polymeric materials are very unique in chemical compo-
sition, physical forms, mechanical properties and applica- smaller molecules, e.g., oligomers, dimers, and monomers,
tions. High versatility of the carbon to carbon and carbon that are smaller enough to pass the semi-permeable outer
to non-carbon (C–C, C–R and C–H) bonds and substituent bacterial membranes, and then to be utilized as carbon and
groups, the possible conÿgurations, stereochemistry and ori- energy sources (Fig. 1). The process is called depolymer-
entation provide basis for variations of chemical structures ization. When the end products are inorganic species, e.g.,
and stereochemistry (Odian, 1991). Very small variations CO2 , H2 O, or CH4 , the degradation is called mineraliza-
in the chemical structures may result in large di erences tion. A commonly recognized rule is that the closer the
in term of biodegradability. Because of this structural ver- similarity of a polymeric structure to a natural molecule,
satility, they are widely used in product packaging, insu- the easier it is to be degraded and mineralized. Polymers
lation, structural components, protective coatings, medical like cellulose, chitin, pullusan, and PHB are all biologically
implants, drug delivery carriers, slow-release capsules, synthesized and can be completely and rapidly biodegraded
electronic insulation, telecommunication, aviation and space by heterotrophic microorganisms in a wide range of natural
industries, sporting and recreational equipment, building e
environment (BÃ renger et al., 1985; Byrom, 1991; Chahal
consolidants, etc. In service, they are constantly exposed to et al., 1992; Frazer, 1994; Gamerith et al., 1992; Gujer
a range of natural and artiÿcial conditions often involving and Zehnder, 1983; Gunjala and Sul ita, 1993; Hamilton
microbial contamination, resulting in aging, disintegra- et al., 1995; Hass et al., 1992; Hespell and O’Bryan-Shah,
tion, and deterioration over time (Lemaire et al., 1992; 1988; Kormelink and Voragen, 1993; Lee et al., 1985,
Pitt, 1992). 1987a, b, 1993; Luthi et al., 1990a, b; MacDonald et al.,
1985; MacKenzie et al., 1987; Nakanishi et al., 1992;
Sonne-Hansen et al., 1993; Sternberg et al., 1977; Torronen
3.1. Microorganisms and general degradation et al., 1993; Wong et al., 1988; Yoshizako et al., 1992).
In addition, natural conditions also include environments
Polymers are potential substrates for heterotrophic where anaerobic processes are the leading ones (Brune et
microorganisms including bacteria and fungi. Polymer al., 2000; Fenchel and Finlay, 1995). Under such conditions,
biodegradability depends on molecular weight, crystallinity the complete decomposition of a polymer will produce or-
and physical forms (Gu et al., 2000b). Generally, an in- ganic acids, CO2 , CH4 and H2 O. It is important to note that
crease in molecular weight results in a decline of polymer biodeterioration and degradation of polymer substrate can
degradability by microorganisms. In contrast, monomers, rarely reach 100% and the reason is that a small portion of
dimers, and oligomers of a polymer’s repeating units are the polymer will be incorporated into microbial biomass,
much easily degraded and mineralized. High molecular humus and other natural products (Alexander, 1977; Atlas
weights result in a sharp decrease in solubility making them and Bartha, 1997; Narayan, 1993).
unfavorable for microbial attack because bacteria require Dominant groups of microorganisms and the degradative
the substrate be assimilated through the cellular membrane pathways associated with polymer degradation are often
and then further degraded by cellular enzymes. However, it determined by the environmental conditions. When O2 is
should be pointed out that concurrent abiological and bio- available, aerobic microorganisms are mostly responsi-
logical processes may facilitate the degradation of polymers. ble for destruction of complex materials, with microbial
At least two categories of enzymes are actively involved biomass, CO2 , and H2 O as the ÿnal products (Fig. 1). In
in biological degradation of polymers: extracellular and contrast, under anoxic conditions, anaerobic consortia of
intracellular depolymerases (Doi, 1990; Gu et al., 2000b). microorganisms are responsible for polymer deterioration.
During degradation, exoenzymes from microorganisms The primary products will be microbial biomass, CO2 , CH4
break down complex polymers yielding short chains or and H2 O under methanogenic conditions (Barlaz et al.,
72 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
1989a, b; Gu et al., 2000e, 2001; Gu and Mitchell, 2001) and the environmental conditions. High molecular weight
or H2 S, CO2 and H2 O under sulÿdogenic conditions polymers are less biodegradable or degraded at a slower
(Fig. 1). It is known that aerobic processes yield much rate than those with low molecular weights. For example,
more energy and are capable of supporting a greater popu- the rate of hydrolytic chain cleavage of ester bonds in the
lation of microorganisms than anaerobic processes because following polymers is dependent on the co-polymer com-
thermodynamically O2 is a more e cient electron acceptor position: poly(3-hydroxybutyrate-co-27% 4-hydroxybuty-
than SO2− and CO2 . These conditions are widely found
4 rate) [P(3HB-co-27% 4HB)]¿[P(3HB-co-17% 4HB)]¿
in natural environments and can be simulated in the labo- [P(3HB-co-10% 4HB)]¿ poly(3-hydroxybutyrate-co-
ratory with appropriate inocula. Both aerobic and strictly 45% 3-hydroxybutyrate [P(3HB-co-45% 3HV)]¿[P(3HB-
anaerobic microorganisms are involved in the degradation co-71% 3HV)] (Doi, 1990). Similarly, the sequence of enzy-
of polymers. matic hydrolysis is [P(HB-co-16% HV)]¿[P(HB-co-32%
In this review, synthetic polymers are divided into three HV)]¿PHB (Parikh et al., 1993). In addition, crystallinity
groups: (1) degradable, (2) slowly degradable, and (3) re- and stereochemistry of polymers also a ect the rate of
sistant. Natural polymers, e.g., cellulose, chitin, chitosan, degradation signiÿcantly, but is rarely taken into account
lignin, and polysaccharides, etc. are excluded. (Budwill et al., 1992; Gu et al., 2000b,e). This characteris-
tic of molecules and its e ects on degradation has received
attention recently (Kohler et al., 2000).
3.2. Biodeterioration of polymers
3.2.1. Microbiologically synthesized polymers 3.2.2. Poly(ÿ-hydroxyalkanoates)
Microorganisms are capable of manufacturing a range of Bacterial poly(ÿ-hydroxyalkanoates) are formed dur-
complex polymers under conditions when excessive carbon ing nutrient limited growth when the carbon source is in
source is available, e.g., C/N 10. The polymers include a excess, e.g., high C/N ratio, as energy storage materials
diverse class of polyesters (Doi, 1990; Stenbuchel, 1991), (Anderson and Dowes, 1990; Brandl et al., 1988; Doi,
polysaccharides (Linton et al., 1991), silk (Kaplan et al., 1990; Holmes et al., 1985; Kim et al., 1995; Lemoigne,
1991). Microbial degradation of polymers depends on their 1926; Stenbuchel, 1991). Under condition of nutrient lim-
molecular compositions, molecular weights and the pres- itation, these materials can be depolymerized and utilized
ence of speciÿc microorganisms on surfaces of materials. by microorganisms. They consist of homo or co-polymers
Some can be almost completely utilized as a source of car- of [R]-ÿ-hydroxyalkanoic acids. This polymer is a micro-
bon and energy while others are only partially degraded. Ex- bial intracellular inclusion in the cytoplasmic uid in the
amples of the former include the poly(hydroxyalkanoate)s form of granules with diameters between 0.3 and 1:0 m
(PHAs) (Anderson and Dowes, 1990; Brandl et al., 1988; (Stenbuchel, 1991). Biopolymers may comprise as much
Choi and Yoon, 1994; Doi, 1990; Nakayama et al., 1985; as 30 –80% of the total cellular biomass. The polymer has
Stenbuchel, 1991; Stuart et al., 1995; Tanio et al., 1982); been isolated from Bacillus megaterium by extraction in
-poly(glutamic acid) (Cromwick and Gross, 1995), cellu- chloroform and has a molecular weight of approximately
lose acetates with degree of substitution values lower than 105 –106 with more than 50% in crystalline form (Gu et
2.5 (Buchanan et al., 1993; Gross et al., 1993, 1995; Gu al., unpublished data). Unlike other biopolymers, such as
et al., 1992b, c, 1993a–c, 1994b), polyethers (Kawai, 1987; polysaccharides, proteins and DNAs, PHB is thermoplas-
Kawai and Moriya, 1991; Kawai and Yamanaka, 1986), tic with a melting temperature around 180◦ C, making it a
polylactide (Gu et al., 1992b,c), polyurethanes (Blake et good candidate for thermoprocessing. Furthermore, PHB
al., 1998; Crabbe et al., 1994; El-Sayed et al., 1996; Filip, and co-polymers have also been produced in genetic engi-
1978; Gillatt, 1990; Gu et al., 1998b; Mitchell et al., 1996; neered plants (John and Keller, 1996) and through chemical
Nakajima-Kambe et al., 1995; Szycher, 1989), and natural synthesis (Kemnitzer et al., 1992, 1993), which provide
rubbers (Berekaa et al., 2000; Heisey and Papadatos, 1995). potential for commercial production in the future.
Chemical structure of a polymer determines the ex- Both homopolymers and co-polymers can be degraded un-
tent of biodegradation. A general rule is that biologically der biologically active environments, e.g., soil (Albertsson
synthesized polymers are readily biodegradable in natu- a
et al., 1987; Mas-CastellÂ et al., 1995; Tsao et al., 1993),
ral environments and synthetic polymers are either less sludge, compost (Gilmore et al., 1992, 1993; Gross et al.,
biodegradable or degraded very slowly. This widely ac- 1993, 1995; Gu et al., 1993b), river water (Andrady et al.,
cepted rule suggests that the degradation processes have 1993; Imam et al., 1992) and seawater (Andrady et al.,
evolved through time and complexity of biochemical path- 1993; Imam et al., 1999; Sullivan et al., 1993; Wirsen and
ways may increase with the structure diversiÿcation of Jannasch, 1993). Extracellular PHB depolymerases have
polymeric materials. However, the rate of degradation is been isolated from Pseudomonas lemoignei (Lusty and
largely a ected by the chemical structure, e.g., the C–C Doudoro , 1966) and A. faecalis (Saito et al., 1989; Tanio
and other types of bonds, molecular weights, structures and et al., 1982). Other bacteria capable of degrading these poly-
conÿguration as well as the participating microorganisms mers include Acidovorax facilis, Variovorax paradoxus,
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 73
Fig. 2. Scanning electron micrographs of (a) aerobic soil bacteria growing on surface of poly-ÿ-hydroxybutyrate (PHB) (scale bar, 10 m) and (b)
bacteria surrounding a PHB granule after incubation under mesophilic conditions (35◦ C) (scale bar, 5 m).
Pseudomonas syringae subsp. savastanoi, Comamonas and mechanical properties for di erent applications (Bogan
testosteroni, Cytophaga johnsonae, Bacillus megaterium, and Brewer, 1985). Because the backbone is natural cellu-
B. polymyxa, and Streptomyces spp. (Mergaert et al., lose, theoretically they can carry substitution values from as
1993). The enzymatic degradation occurs initially at the low as near zero to as high as 3.0. Current knowledge is that
surfaces of the polyester ÿlm after microbial colonization CAs with a degree of substitution values less than 2.5 can
(Fig. 2), and the rate of surface erosion is highly dependent be degraded in thermophilic compost (Gross et al., 1993,
on both the molecular weight (degree of polymerization), 1995; Gu et al., 1992b, c, 1993a–c, 1994b) or transformed
composition of the polyester, crystallinity and the dominant to solvents through biological catalyzed reactions (Downing
species of bacteria. et al., 1987). Apparently, increasing the DS value makes
the polymers less degradable. As discussed above, it is clear
3.3. Modiÿed natural polymers that slightly deviation from the natural structures will lead
to increasing resistance to deterioration and degradation.
3.3.1. Cellulose acetates (CAs) CA degradation occurs more rapidly under oxic condi-
Cellulose acetates (CAs) are a class of natural polymers tions than anoxic conditions. The mechanisms of initial
with chemical modiÿcation to improve their processibility degradation reaction are de-acetylation, which releases the
74 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Fig. 3. Scanning electron micrograph showing bacteria growing on surfaces of cellulose acetate.
substituted groups, followed by cleavage of the C–C clude polyethylene glycols (PEGs), polypropylene glycols
backbone. In this case, substituting group has a strong (PPGs) and polytetramethylene glycol (PTMGs). They are
in uence on the degradability of polymer. It is also demon- used in pharmaceuticals, cosmetics, lubricants, inks, and sur-
strated recently that the decrease of molecular weight by factants. Contamination of natural waters, including coastal
cleavage of C–C chain and de-acetylation proceed simul- waters and streams where wastewater is discharged have
taneously during degradation after CA reaches to a critical been reported (Kawai, 1987, 2002).
value of substitution of approximately 1.0. Structural substi- Degradability of this class of polymers has been studied
tution groups, and their numbers per repeating unit, a ects under both oxic (Kawai, 1987, 2002; Kawai and Moriya,
the degradation kinetics remarkably. For example, cellulose 1991; Kawai and Yamanaka, 1986) and anoxic conditions
acetate (CA) with a lower degree of substitution (DS) value (Dwyer and Tiedje, 1983; Frings et al., 1992; Schink and
is more quickly degraded than those with higher substitution Stieb, 1983). Their degradability is highly dependent on
values under both oxic and anoxic conditions (Buchanan molecular weight. Molecules with molecular weights higher
et al., 1993; Gross et al., 1993, 1995; Gu et al., 1992b, c, than 1000 have been considered resistant to biodegradation
1993a–c, 1994b) (Fig. 3). CAs with lower substitution val- (Kawai, 1987). However, degradation of PEGs with molec-
ues (∼ 0:82) also show relatively higher solubility which
= ular weights up to 20,000 has been reported (Kawai and
is favored by microbial metabolism. During degradation of Yamanaka, 1989). The ability of a micro ora to degrade
CA, both molecular weight and degree of substitution de- PEG molecules with high molecular weights is dependent
creased, suggesting that de-acetylation and decomposition primarily on the ability of a syntrophic association of di er-
of the polymer backbone proceed simultaneously (Gu et al., ent bacteria to metabolize the chemicals (Fig. 4). For exam-
1993c). Earlier data also suggested that CA with DS values ple, Flavobacterium sp. and Pseudomonas sp. can form an
greater than 0.82 are recalcitrant to biodegradation and that e ective association and mineralize PEG completely. Dur-
the limiting step is de-acetylation, followed by breaking of ing degradation, PEG molecules are reduced by one glycol
the polymer carbon–carbon bonds (Reese, 1957). Current unit after each oxidation cycle.
results showing degradation of CA indicated that CA degra- The central pathway of PEG degradation is cleavage of
dation has been observed with DS values as high as 2.5. an aliphatic ether linkage. In a co-culture of aerobic Flavo-
Microorganisms capable of CA degradation are mostly bacterium and Pseudomonas species, PEG degradation pro-
actinomyces, fungi and selective bacteria (Gross et al., 1993, ceeds through dehydrogenation to form an aldehyde and
1995; Gu et al., 1992b, c, 1993a–c). One bacterium Pseudo- a further dehydrogenation to a carboxylic acid derivative
monas paucimobilis was isolated for ability to degrade CA (Kawai, 1987; Kawai and Yamanaka, 1986). It is important
with DS value 1.7 from a composting bioreactor containing to note that either of the two bacteria in pure culture cannot
CA ÿlms (Gross et al., 1993). degrade PEG alone. Cellular contact between them seems
to be essential for e ective activity (Kawai, 1987).
3.4. Synthetic polymers In the investigated Flavobaterium sp. and Pseudomonas
sp. system, three enzymes are involved in the complete
3.4.1. Polyethers degradation of PEG (Kawai, 1987). PEG dehydrogenase,
One of the most commonly used synthetic polymers with PEG-aldehyde dehydrogenase, and PEG-carboxylate de-
wide application and usage is polyethers. The polymers in- hydrogenase (ether-cleaving) are all required. All of them
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 75
Fig. 4. Scanning electron micrograph showing a pure culture of bacteria capable of utilizing polyethylene glycol as a source of carbon and energy.
are found in Flavobaterium sp., while only PEG-carboxylate aircraft structures, due to their exibility and compressive
dehydrogenase is present in Pseudomonas sp. Using PEG strength. They are also used in appliance construction, cook-
6000 as a sole substrate no degradation can be observed with ingware, and food packaging because of their chemical re-
either of the two bacteria alone. In addition, the ether cleav- sistance to oils, greases, and fats, microwave transparency,
age is extremely sensitive to the presence of glycoxylic acid. and thermal resistance. Their electrical insulation properties
However, Pseudomonas sp. though not directly involved are ideally suited for use in the electrical and electronics
in the degradation, is capable of utilizing the toxic meta- markets, especially as high temperature insulation materials
bolite that inhibits the activity of the Flavobacterium sp. and passivation layers in the fabrication of integrated cir-
This connection appears to be the essential link for their cuits and exible circuitry. In addition, the ammability re-
closely syntrophic association in achieving completely sistance of this class of polymers may provide a halogen-free
degradation of PEG. ame-retardant material for aircraft interiors, furnishings,
Under anaerobic condition, EG, PEG can also be degraded and wire insulation. Other possible uses may include ÿbers
(Dwyer and Tiedje, 1983) but only one bacterium Pelo- for protective clothing, advanced composite structures, ad-
bacter venetianus was reported (Schink and Stieb, 1983). hesives, insulation tapes, foam, and optics operating at high
temperatures (Verbiest et al., 1995).
Electronic packaging polyimides are particularly useful
3.5. Recalcitrant polymers because of their outstanding performance and engineering
properties. It is only recently that biodeterioration of these
3.5.1. Electronic insulation polyimides polymers was investigated using pyromellitic dianhydride
Polymers used in electronic industries are chemically syn- and 4; 4 -diaminodiphenyl ether with molecular weight (Mw
thesized with the objective of high strength and resistance of 2:5 × 105 ) (Ford et al., 1995; Gu et al., 1994a, 1995a,
to degradation. Thermosetting polyimides are major class in 1996b, c, 1998a, b; Mitton et al., 1993, 1996, 1998). They
this application (Brown, 1982). Wide acceptance of poly- are susceptible to deterioration by fungi (Fig. 5) (Ford et
imides in the electronics industry (Brown, 1982; Jensen, al., 1995; Gu et al., 1994a, 1995a, 1996b; Mitton et al.,
1987; Lai, 1989; Verbicky, 1988; Verbiest et al., 1995) 1993, 1998). Though bacteria were isolated from culture
has drawn attention to the stability of these materials. The containing the deteriorated polyimides, further tests did not
National Research Council (NRC, 1987) emphasized the show comparable degradation by bacteria.
need to apply these polymers in the electronic industries be- Our studies showed that the dielectric properties of poly-
cause data acquisition, information processing and commu- imides could be altered drastically following growth of a
nication are critically dependent on materials performance. microbial bioÿlm (Ford et al., 1995; Gu et al., 1995a, 1996b;
The interlayering of polyimides and electronics in integrated Mitton et al., 1993, 1998). This form of deterioration may
circuits prompted several studies on the interactions between be slow under ambient conditions. However, the deteriora-
these two materials (Hahn et al., 1985; Kelley et al., 1987). tion processes can be accelerated in humid conditions or in
Polyimides are also widely used in load bearing applica- enclosed environments, e.g., submarines, space vehicles,
tions, e.g., struts, chasses, and brackets in automotive and aircraft, and other closed facilities. Very small changes of
76 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Fig. 5. Photograph and scanning electron micrograph showing: (a) the visible colonization of microorganisms in the inoculated cell containing polyimides
and (b) the microorganisms colonizing and growing on the surface of polyimides.
material insulation properties may result in serious and Initial isolation of microorganisms associated with dete-
catastrophic consequences of communications and control rioration of polyimides indicated the presence of both fungi
systems. and bacteria. Bacteria include Acinetobacter johnsonii,
Polyimide deterioration occurs through bioÿlm forma- Agrobacterium radiobacter, Alcaligenes denitriÿcans,
tion and subsequent physical changes in the polymer. Using Comamonas acidovorans, Pseudomonas spp, and Vibrio
electrochemical impedance spectroscopy (EIS) (Mansfeld, anguillarum. These bacteria were not capable of degrad-
1995; van Westing et al., 1994), a very sensitive tech- ing the polymer after inoculation while fungi were more
nique for monitoring dielectric constant of polymers, fungal e ective in degrading the polyimides.
growth on polyimides have been shown to yield distinctive
EIS spectra, indicative of failing resistivity. In the degra- 3.5.2. Fiber-reinforced polymeric composite materials
dation processes, two steps are involved during degrada- Fiber-reinforced polymeric composite materials (FR-
tion: an initial decline in coating resistance is related to the PCMs) are newly developed materials important to
partial ingress of water and ionic species into the polymer aerospace and aviation industries (Gu et al., 1994a, 1995a–d,
matrices. This is followed by further deterioration of the 1996a, 1997a, b; Wagner, 1995; Wagner et al., 1996). The
polymer by activity of the fungi, resulting in a large decrease increasing usage of FRPCMs as structural components of
in resistivity. Fungi involved include Aspergillus versicolor, public structures and particularly in aerospace application
Cladosporium cladosporioides, and Chaetomium sp. (Gu has generated an urgent need to evaluate the biodegrad-
et al., 1995a, 1996a, e, 1997a, b, 1998a). The data support ability of this class of new materials. FRPCMs are also
the hypothesis that polyimides are susceptible to microbial susceptible to attack by microorganisms (Gu et al., 1997b).
deterioration and also conÿrm the versatility of EIS as a It was suggested that impurities and additives that can pro-
method in evaluation of the biosusceptibility of polymers. mote microbial growth are implicated as potential sources
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 77
Fig. 6. Scanning electron micrographs showing colonization of surfaces of: (a) ÿber-reinforced polymeric composite by both bacteria and fungi and (b)
graphite carbon ÿbers by mostly fungi.
of carbon and energy for the environmental microorganisms teria and fungi are capable of growing on the graphite
(Fig. 6). ÿbers of FRPCMs, but only fungi have been shown to
In this area of research, two groups reported microbial cause deterioration detectable over more than 350 days (Gu
degradation of FRPCMs (Gu and Mitchell, 1995; Gu et al., et al., 1995b, 1997a, b). It was also found that plasticizers
1995b–d, 1996a, 1997a, b; Wagner et al., 1996). A mixed are biodegradable and utilized by natural microorganisms
culture of bacteria including a sulfate-reducing bacterium as source of carbon and energy (Gu et al., 1994a, 1996a).
was used to show the material deterioration (Wagner et al., Phthalate and phthalate esters are the largely groups of
1996). In contrast, Gu et al. (1994a, 1996a–c, 1997a, b) chemicals used as plasticizers in plastics manufacturing,
used a fungal consortium originally isolated from degraded they are also detected at high concentrations in landÿll
polymers and a range of material composition including leachate (Mersiosky, 2002) and degraded by aerobic mi-
uorinated polyimide/glass ÿbers, bismaleimide/graphite croorganisms quickly (Fan et al., 2001; Wang et al., 2003).
ÿbers, poly(ether-ether-ketone) (PEEK)/graphite ÿbers, Physical and mechanical tests were not su ciently sensitive
and epoxy/graphite ÿbers (Gu et al., 1995b). The fungal to detect any signiÿcant physical changes in the materials
consortium consisted of Aspergillus versicolor, Clado- after the duration of exposure (Gu et al., 1997b; Thorp
sporium cladosorioides, and a Chaetomium sp. Both bac- et al., 1994). However, the resins were actively degraded,
78 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Fig. 7. Scanning electron micrograph of a pure culture of bacteria capable of degrading water-soluble polyurethane.
indicating that the materials were at risk of failure. It is clear Similar to the microorganisms isolated from polyimides,
that both ÿber surface treatment and resin processing supply bacteria are less e ective in degrading the composites than
enough carbon for microbial growth (Gu et al., 1995d). It fungi (Gu et al., 1995b). Degradation of composites were
has become clear that FRPCMs are not immune to adhesion detected using electrochemical impedance spectroscopy.
and attack by microorganisms (Ezeonu et al., 1994a,b; Gu
et al., 1998b; Mitchell et al., 1996). 3.5.3. Corrosion protective polymers
Natural populations of microorganisms are capable of Corrosion protective coatings also have wide applica-
growth on surfaces of FRCPM coupons at both relatively tion because the development of metallic materials and
high (65 –70%) and lower humidity conditions (55 – 65%) susceptibility to corrosion both environmentally and micro-
(Gu et al., 1998b). The accumulation of fungi on surfaces of biologically (Mitchell et al., 1996). Polymeric coatings are
composites develops into a thick bioÿlm layer and decreases designed to prevent contact of the underlying materials with
the resistance to further environmental changes. However, corrosive media and microorganisms. However, microbial
the resistivity of FRPCMs was found to decline signiÿcantly degradation of coatings may accelerate and severely dam-
after the initial 3 months during a year of monitoring using age the underlying metals. Typical example includes the
EIS (Gu et al., 1996c, 1997b). Clear di erences resulting corrosion of underground storage tanks. Natural bacterial
from bioÿlm development were detected on FRCPMs used populations were found to readily form microbial bioÿlms
in aerospace applications (Gu et al., 1997b). Further study on surfaces of coating materials, including epoxy and
indicated that many fungi are capable of utilizing chemicals, polyamide primers and aliphatic polyurethanes (Blake et al.,
e.g., plasticizers, surface treatment chemicals and impurities, 1998; Filip, 1978; Gu et al., 1998b; Stern and Howard,
introduced during composite manufacture as carbon and en- 2000; Thorp et al., 1997) (Fig. 7). Surprisingly, the addition
ergy sources (Gu et al., 1996a). Similarly, lignopolystyrene of biocide diiodomethyl-p-tolylsulfone into polyurethane
graft copolymers were also susceptible to attack by fungi coatings did not inhibit bacterial attachment or growth
(Milstein et al., 1992). of bacteria e ectively due to development of bioÿlm and
A critical question remains about the e ect of FRPCM bacterial resistance (Gu et al., 1998b; Mitchell et al., 1996).
deterioration on mechanical properties of the composite ma- Using EIS, both primers and aliphatic polyurethane
terials. Thorp et al. (1994) attempted to determine mechani- top-coatings were monitored for their response to biodegra-
cal changes in composite coupons after exposure to a fungal dation by bacteria and fungi. Results indicated that primers
culture. No signiÿcant mechanical changes could be mea- are more susceptible to degradation than polyurethane
sured after 120 days exposure. They suggested that method- (Gu et al., 1998b). The degradation process has similar
ologies su ciently sensitive to detect surface changes need mechanisms as polyimides and FRPCMs as mentioned
to be utilized. Acoustic techniques have also been proposed above. Aliphatic polyurethane-degrading bacteria have been
as a means of detecting changes in the physical properties isolated and one of them is Rhodococcus globerulus P1
of the FRPCMs (Wagner et al., 1996). base on 16S rRNA sequence (Gu, unpublished data).
Many bacteria were capable of growth on surfaces of FR- Polyurethane-degrading microorganisms including
PCMs and resins (Gu et al., 1996a). The bacteria are be- Fusarium solani, Curvularia senegalensis, Aureobasidium
lieved to be introduced onto the polymers during production. pullulans and Cladosporidium sp were isolated (Crabbe
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 79
et al., 1994) and esterase activity was detected with
C. senegalensis. A number of bacteria were also claimed
to be capable of degrading polyurethane and they are four
stains of Acinetobacter calcoaceticus, Arthrobacter glob-
iformis, Pseudomonas aeruginosa, Pseudomonas cepacia,
Pseudomonas putida, and two other Pseudomonas-like
species (El-Sayed et al., 1996). A Comamonas aci-
dovoran TB-35 was also reported (Akutsu et al., 1998;
Nakajima-Kambe et al., 1995, 1997). In addition, Pseu-
domonas chlororaphis was isolated and encoded a lipase
responsible for the degradation (Stern and Howard, 2000).
3.6. Resistance polymers
Polyethylenes (PEs) of high and low density are primar-
ily used in product packaging as sheets and thin ÿlms. Their
degradability in natural environments poses serious environ-
mental concerns due to their slow degradation rates under
Fig. 8. Photographs showing the: (a) ancient writing script, (b) textile,
natural conditions, and the hazard they present to freshwater (c) bronze, and (d) books with molding development from a library in
and marine animals. Prior exposure of PEs to UV promotes the tropical region.
polymer degradation. It is believed that polymer additives,
such as starch, antioxidants, coloring agents, sensitizers, and
plasticizers may signiÿcantly alter the biodegradability of At higher temperatures, ketones, alcohols, aldehydes, lac-
the parent polymers (Karlsson et al., 1988). Degradation tones, and carboxylic acids are formed abiotically in 6 weeks
rates may be increased by 2– 4% following photosensitizer (Albertsson et al., 1994). PE pipes used in gas distribution
addition. However, degradation is very slow, estimated in systems may fail due to cracking. It is unlikely that biolog-
decades. Crystallinity, surface treatment, additives, molec- ical processes are involved (Zhou and Brown, 1995).
ular weight, and surfactants are all factors a ecting the fate
and rate of PE degradation, and may accelerate the process. 3.6.2. Polypropylenes
Biodegradation of PEs has been studied extensively ear- Polypropylenes (PPs) are also widely utilized as engi-
lier (Albertsson, 1980; Breslin, 1993; Breslin and Swanson, neering pipes and containers. Degradation of PPs results in
1993; Imam and Gould, 1990), but the results were based on a decrease of their tensile strength and molecular weight.
PE blent with starch. For example, extracellular concentrates The mechanism may involve the formation of hydroperox-
of three Streptomyces species cultures were inoculated to ides which destabalize the polymeric carbon chain to form a
starch containing PE ÿlms (Pometto et al., 1992, 1993). Sub- carbonyl group (Cacciari et al., 1993; Severini et al., 1988).
sequently, PE was claimed to be degraded. Realizing that Degradability of pure and high molecular weight PPs is still
degradation may occur and the extent could be extremely an open question.
small, conclusion on PE degradation should be treated with
caution. Other data describing degradation of PE containing
starch is questionable, and microbial metabolites may con- 4. Biodeterioration of cultural heritage materials
taminate the PE surfaces and could be interpreted as degra-
dation products of the parent PE. Abiotic degradation of PE Other materials of interest and importance to society for
is evident by the appearance of carbonyl functional groups protection from biodeterioration are cultural objects with
in abiotic environments. In contrast, an increase of double historical and cultural value. Examples of these materials are
bonds was observed when polymers showed weight loss re- bronze (Wang et al., 1991, 1993; Wu et al., 1992; Zou et al.,
sulting from biodegradation (Albertsson et al., 1994). It was 1994), jade, ceramic and glass (Fuchs et al., 1991; Lauwers
proposed that microbial PE degradation is a two-step pro- and Heinen, 1974), lacquer, silk, papers (Adamo et al., 1998;
cess involving an initial abiotic photooxidation, followed by Arai, 2000; Fabbri et al., 1997; Florian, 1996; Zyska, 1996),
a cleavage of the polymer carbon backbone. However, the n
paintings (Fabbri et al., 1997; Pi˜ ar et al., 2001; Rolleke
mechanism of the second step needs extensive analysis be- et al., 1998), animal bones and shells, wood (Blanchette,
fore plausible conclusions can be drawn conÿdently. Lower 1995; King and Eggins, 1972), and mummiÿed bodies.
molecular weight PEs including para n can be biodegraded Fig. 8 shows ancient script on paper and textile, which have
and para n undergoes hydroxylation oxidatively to form been held in museum condition, and modern books from
an alcohol group, followed by formation of carboxylic acid. library in tropic region. These materials are either in need
80 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Fig. 9. Photograph showing inhibition of microorganisms on surface of agar plates by a biocide in the discs placed on the agar plates.
for protection or su er from potential biodeterioration due servation of art works, the e ectiveness of the addition is
to the growth of microorganisms which have been estab- questionable from our past experience (Fig. 9). This prob-
lished their population on surfaces of materials. lem will be more serious than expected when eradication of
Signiÿcant importance for protection and preservation of microorganisms becomes harder using these chemicals due
them is on the social, culture, and archaeological and his- to resistant development in microorganisms after exposure
torical value and scholarly meaning for future study. Con- (Bingaman and Willingham, 1994).
servation and preservation of them are a major task in all
museums worldwide and integrated research e ort deserves
more attention in understanding the processes contributing 5. Prevention and detection of biodeterioration
to the problem and proposing preventive measure or so-
lution. Apparently, such understanding and the preventive 5.1. Preventive measures
measure can only be achieved by collective research e ort
from biologists, chemists and conservators. Microbial growth and propagation on material surfaces
can be controlled by physical and chemical manipulations
4.1. Consolidant polymers of the material and the artiÿcial environments. Preven-
tion against biodeterioration include surface engineering
In addition to the polymers and applications described so that attachment by and susceptibility to microorganisms
above, organic polymers are widely used in consolidation and then the fouling organisms can be reduced greatly
of monuments and repairing of art works (Selwitz, 1992). (Gu and Cheung, 2001; Mansfeld, 1994; Matamala et al.,
Utilization of these materials by common ora of micro- 1994; Scamans et al., 1989; Williamson, 1994; Young,
organisms transported in the atmosphere has been docu- 1948). Basic information on microorganisms are widely
mented (Gu and Mitchell, unpublished data) and guidelines available from textbook (e.g., Madigan et al., 2000) and
are needed for systematic evaluation of candidate polymers microbiological manuals (Balow et al., 1992; Krieg and
and their suitability in speciÿc applications. Since these Holt, 1984; Sneath et al., 1986; Staley et al., 1989; Williams
polymers are mostly commercial products, polymer addi- et al., 1989). As a control measure, lowering humidity
tives and other constituents are more likely to serve as a is a very e ective means to slow down the growth of
source of carbon and energy for microbial growth when tem- microorganisms on surfaces in an enclosed environment
perature and moisture (humidity) are favorable for the prolif- (Gu et al., 1998b) and prevention against potential con-
eration of microorganisms (Gu et al., 1998b, 2000b; Tilstra tamination will prolong the life time of the objects. Under
and Johnsonbaugh, 1993). Even organic pollutants can be museum conditions, sensitive art pieces should be care-
degraded by natural microorganisms (Gu and Berry, 1991, fully protected environmentally and the numbers of visitors
1992; Gu et al., 1992a). These physical conditions are gen- should also be controlled to maintain a relatively constant
erally available particularly in developing countries where temperature and humidity, and to decrease chance of con-
resource is limited for preservation and conservation. tamination.
Among several consolidants including acryloids, Basic measures in control of biodeterioration should be
polyurethane, and epoxies, none of them is resistance to focused on the surface especially the initial population of
microbial colonization (Gu, unpublished data). Though ap- organisms. Without a better understanding of what is on
plication of biocides becomes a routine practice in the con- the surface, subsequent protection measure cannot be tar-
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 81
get speciÿc. In this area, recent development in molecular of assaying e cacy of biocide should be conducted based
technique involving DNA based information allows a bet- on bioÿlm condition than liquid culture e cacy (Gu et al.,
ter examination of any surface due to the shortcomings with 1998b, 2000d). This major discrepancy has not fully been
traditional microbiological techniques (Amann et al., 1995). resolved. Because bioÿlm bacteria are more resistance to an-
Coupling the understanding of surface microbial ecology tibiotics and biocides, tests based on planktonic cells are not
using molecular techniques and then controlling measure, truly representative of their actual conditions on surfaces of
better results can be achieved. By modiÿcation of the micro- materials. New initiative is needed for innovative methodol-
bial community, Sand et al. (1991) proposed oxygenation ogy to assess biocidal e ects using surface oriented assays.
as a means of alleviating the propagation of SRBs under
anoxic conditions. At the same time, biocides can be e ec- 5.3. Testing methodologies
tive in controlling bioÿlms and subsequent deterioration of
materials to some extent (Bell and Chadwick, 1994; Bell Another critical issue in this area is the standardization of
et al., 1992; Wakeÿeld, 1997). Other attempts at community test methodologies. Current available methods are certainly
modiÿcation include precipitation of microbially produced not representative of the actual conditions for each individ-
H2 S by ferrous chloride (FeCl2 ) (Morton et al., 1991), and ual case, but very little exibility is o ered in the methods.
displacement of Thiobacillus sp. by heterotrophic bacteria Simulation testing of microbial growth on materials includes
(Padival et al., 1995). All of these e orts have met with only a small selection of fungal species (ASTM, 1993a–e)
limited success. while deterioration under natural environment is hardly car-
ried out by those species. Furthermore, biodeterioration as-
sessment has hardly been quantitative because presence of
5.2. Use of biocides bacteria or fungi on surface of materials has generally been
assumed as biodeterioration (Zachary et al., 1980). Actu-
Biocides are commonly applied in repairing, cleaning and ally, the interpretation is about the potential for biodeteriora-
maintenance of artworks. Chlorine, iodine and other organic tion not actually biodeterioration and biodegradation. More
biocidal compounds are used widely and routinely in con- methods are now becoming available for test the biodeterio-
trolling bioÿlms which cause corrosion and deterioration ration and biodegradation of organic materials, particularly
of a wide range of materials in industries (Bloomÿeld and polymers in various chemical composition and degradabil-
Megid, 1994; Cargill et al., 1992; Chen and Stewart, 1996; ity (Gross et al., 1993, 1995; Gu et al., 1992b, c, 1993a–c,
Stewart et al., 1996) and conservation of art (Bianchi et al., 1994b, 2000b, d). Both gravimetric method and respiro-
1980; Bingaman and Willingham, 1994). These chemicals metry have been tested and used successfully with CAs and
have been shown to be ine ective in killing bioÿlm bacteria PHB as testing polymers. Highly sensitive and quantitative
(Gu et al., 1998b; Huang et al., 1996; Keevil and Macker- method has also been introduced in evaluation of polymer
ness, 1990; Koenig et al., 1995; Liu et al., 1998; Lu et al., integrity using EIS (Gu et al., 1998a, 1995a–d, 2000b). With
1984, 1989; McFeters, 1991; McFeters et al., 1995; Moore the latest advances, new techniques should be adopted in
and Postle, 1994; Myers, 1988; Pyle et al., 1992; Reinsel tests according to the characteristics of materials and their
et al., 1996; Rossmoore and Rossmoore, 1993; Srinivasan application environments, so that data generated on the ma-
et al., 1995; Stewart, 1996; Stewart et al., 1996; Suci et al., terials will be a quantitative description of the biological
1998; Wakeÿeld, 1997; Xu et al., 1996; Yu and McFeters, deterioration potential.
1994). In addition to their environmental unacceptability Prevention against bioÿlm formation and biodeterioration
most of the time because of toxicity, biocides induce the de- include surface engineering so that attachment and suscep-
velopment of bioÿlms that are highly resistant to the levels tibility to microorganisms and the fouling organisms can
of chlorine normally utilized to prevent biocorrosion. Or- be reduced greatly (Mansfeld, 1994; Matamala et al., 1994;
ganic biocides, used to prevent bacterial growth in industrial Scamans et al., 1989; Williamson, 1994; Young, 1948).
systems, may selectively enrich population of microorgan- Early detection is an important component in diagnosis and
isms capable of biocide resistance (Fig. 9). No solution to prevention of severe deterioration of materials (Li et al.,
these problems is currently available and alternative biocides 1997). It should also be pointed out that new detection tech-
have been screened from natural products (Abdel-Hafez and nologies including optical ÿber (Bacci, 1995), DNA probes
El-Said, 1997; Bell and Chadwick, 1994; Bell et al., 1992; and microarray (Raychaudhuri et al., 2001; Salama et al.,
Brozel and Cloete, 1993). Current research by materials sci- 2000) will ÿnd valuable applications in this exiciting ÿeld
entists is focused on the prevention of adhesion of corrosive of research and development in the near future.
microorganisms to surfaces through surface treatments and
modiÿcation (Costerton et al., 1988).
Since bacteria are capable of forming bioÿlms on surfaces 6. Conclusions
of materials, future tests should be focused on the dynam-
ics of bioÿlm and quantiÿcation than descriptively showing Microorganisms are involved in the degradation and de-
bioÿlm of scanning electron micrographs. In particular, test terioration of polymers under both aerobic and anaerobic
82 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
conditions. We have only recently begun to understand the Arai, H., 2000. Foxing caused by fungi: twenty-ÿve years of study.
complex nature of interactions between the micro ora and International Biodeterioration & Biodegradation 46, 181–188.
deterioration of polymeric materials. Arino, X., Hernandez-Marine, M., Saiz-Jimenez, C., 1997. Colonization
of Roman tombs by calcifying cyanobacteria. Phycologia 36, 366–373.
Degradation mechanisms are speciÿcally related to the
ASTM (American Society for Testing and Materials), 1993a. Standard
chemical structures, molecular weights, presence of the test method for determining the aerobic biodegradability of degradable
microorganisms and environmental conditions. Protection plastics by speciÿc microorganisms. In: 1993 Annual Book of
of materials can be achieved to some extent through surface ASTM Standards, Vol. 08.03, D5247-92. Philadelphia, Pennsylvania,
engineering and control of the physical, chemical and bio- pp. 401– 404.
logical environments, so that the material surfaces can be as ASTM (American Society for Testing and Materials), 1993b. Standard
test method for assessing the aerobic biodegradation of plastic materials
inert as possible. Application of biocides has been widely
in an activated-sludge-wastewater-treatment system. In: 1993 Annual
used but the development of resistant bacteria is a more Book of ASTM Standards, Vol. 08.03, D5271-92. Philadelphia,
serious problem than even anticipated before. Utilization Pennsylvania, pp. 411– 416.
of molecular techniques to detect speciÿc groups of micro- ASTM (American Society for Testing and Materials), 1993c. Standard
organisms involved in the degradation process will allow test method for determining aerobic biodegradation of plastic materials
a better understanding of the organization of the microbial under controlled composting conditions. In: 1993 Annual Book of
ASTM Standards, Vol. 08.03, D5338-92. Philadelphia, Pennsylvania,
community involved in the attack of materials. Control pp. 444 – 449.
methods should be developed based on the combined infor- ASTM (American Society for Testing and Materials), 1993d. Standard
mation o the material characteristics and microbial specie practice for determining resistance of synthetic polymeric materials to
composition. fungi. In: 1993 Annual Book of ASTM Standards, Vol. 08.03, G21-90.
Philadelphia, Pennsylvania, pp. 527–529.
ASTM (American Society for Testing and Materials), 1993e. Standard
Acknowledgements practice for determining resistance of plastics to bacteria. In: 1993
Annual Book of ASTM Standards, Vol. 08.03, G22-76. Philadelphia,
Pennsylvania, pp. 531–533.
I thank Jessie Lai and Yanzhen Fan for the digitalization
Atlas, R.M., Bartha, R., 1997. Microbial Ecology: Fundamentals and
of images and references. Applications, 4th Edition. Benjamin/Cummings Publishing Company,
Menlo Park, CA.
References Bacci, M., 1995. Fibre optics applications to works of art. Sensors and
Actuators B 29, 190–196.
Balow, A., Truper, H.G., Dworkin, M., Harder, W., Schleifer, K.-H.,
Abdel-Hafez, S.I.I., El-Said, A.H.M., 1997. E ect of garlic, onion and
1992. The prokaryotes. In: A Handbook on the Biology of Bacteria:
sodium benzoate on the myco ora of pepper, cinnamon and rosemary
Ecophysiology, Isolation, identiÿcation, Applications, Vols. I, II, III,
in Egypt. International Biodeteration & Biodegradation 39, 67–97.
Adamo, A.M., Giovannotti, M., Magaudda, G., Plossi ZappalÂ , M., a IV. Springer, New York.
Rocchetti, F., Rossi, G., 1998. E ect of gamma rays on pure cellulose Barlaz, M.A., Ham, R.K., Schaefer, D.M., 1989a. Mass-balance analysis
paper. Restaurator 19, 41–59. of anaerobically decomposed refuse. Journal of Environmental
Akutsu, Y., Nakajima-Kambe, T., Nomura, N., Nakahara, T., 1998. Engineering 115, 1088–1102.
Puriÿcation and properties of a polyester polyurethane-degrading Barlaz, M.A., Schaefer, D.M., Ham, R.K., 1989b. Bacterial population
enzyme from Comamonas acidovorans TB-35. Applied and development and chemical characterization of refuse decomposition in
Environmental Microbiology 64, 62–67. a simulated sanitary landÿll. Applied and Environmental Microbiology
Albertsson, A.-C., 1980. The shape of the biodegradation curve for low 55, 55–65.
and high density polyethylenes in prolonged series of experiments. Becker, T.W., Feumbein, W.E., Warscheid, T., Resende, M.A.,
European Polymer Journal 16, 623–630. 1994. Investigation into microbiology. In: Herkenrath, G.M. (Ed.),
Albertsson, A.-C., Andersson, S.O., Karlsson, S., 1987. The mechanism Investigations into Devices Against Environmental Attack on Stone.
of biodegradation of polyethylene. Polymer Degradation and Stability GKSS-Forschungszentrum Geesthacht, GmbH. Geesthacht, Germany,
18, 73–87. pp. 147–190.
Albertsson, A.-C., Barenstedt, C., Karlsson, S., 1994. Abiotic degradation Bell, G.M., Chadwick, J., 1994. Regulatory controls on biocides in the
products from enhanced environmentally degradable polyethylene. United Kingdom and restrictions on the use of triorganotin-containing
Acta Polymers 45, 97–103. antifouling products. International Biodeterioration & Biodegradation
Alexander, M., 1977. Introduction to Soil Microbiology, 2nd Edition. 34, 375–386.
Wiley, New York.
Bell, E., Dowding, P., Cooper, T.P., 1992. The e ect of a biocide treatment
Amann, R.I., Ludwig, W., Schleifer, K.-H., 1995. Phylogenetic
and a silicone treatment on the weathering of limestone. Environmental
identiÿcation and in situ detection of individual microbial cells without
Technology 13, 687–693.
cultivation. Microbiological Reviews 59, 143–169.
Anderson, A.J., Dowes, E.A., 1990. Occurrence, metabolism, metabolic Berekaa, M.M., Lino, A., Reichelt, R., Keller, U., Steinbuchel, A., 2000.
role, and industrial uses of bacterial polyhydroxyalkanoates. E ect of pretreatment of rubber material on its biodegradability by
Microbiological Reviews 54, 450–472. various rubber degrading bacteria. FEMS Microbiology Letters 184,
Andrady, A.L., Pegram, J.E., Nakatsuka, S., 1993. Studies on enhanced 199–206.
degradable plastics. 1. The geographic variability in outdoor lifetimes e
BÃ renger, J.-F., Frixon, C., Bigliardi, J., Creuzet, N., 1985. Production,
of enhanced photodegradable polyethelenes. Journal of Environmental puriÿcation and properties of thermostable xylanase from Clostridium
Polymer Degradation 1, 31–43. stercorarium. Canadian Journal of Microbiology 31, 635–643.
Angles, M.L., Marshall, K.C., Goodman, A.E., 1993. Plasmid transfer Beveridge, T.J., Makin, S.A., Kadurugamuwa, J.L., Li, Z., 1997.
between marine bacteria in the aqueous phase and bioÿlms in reactor Interactions between bioÿlms and the environment. FEMS
microcosms. Applied and Environmental Microbiology 59, 843–850. Microbiological Reviews 20, 291–303.
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 83
Bianchi, A., Favali, M.A., Barbieri, N., Bassi, M., 1980. The use Busscher, H.J., Sjollema, J., van der Mei, H.C., 1990. Relative
of fungicides on mold-covered frescoes in S. Eusebio in Pavia. importance of surface free energy as a measure of hydrophobicity in
International Biodeterioration Bulletin 16, 45–51. bacterial adhesion to solid surfaces. In: Doyle, R.J., Rosenberg, M.
Bingaman, W.W., Willingham, G.L., 1994. The changing regulatory (Eds.), Microbial Cell Surface Hydrophobicity. American Society for
environment: EPA registration of a new marine antifoulant active Microbiology, Washington, DC, pp. 335–339.
ingredient. International Biodeterioration & Biodegradation 34, Byrom, D., 1991. Miscellaneous biomaterials. In: Byrom, D. (Ed.),
387–399. Biomaterials: Novel Materials from Biological Sources. Macmillan,
Bitton, G., 1980. Adsorption of viruses to surfaces: technological New York, pp. 335–359.
and ecological implications. In: Bitton, G., Marshall, K.C. (Eds.), Cacciari, I., Quatrini, P., Zirletta, G., Mincione, E., Vinciguerra,
Adsorption of Microorganisms to Surfaces. Wiley, New York, V., Lupattelli, P., Sermanni, G.G., 1993. Isotactic polyproplene
pp. 331–374. biodegradation by a microbial community: physicochemical
Blake II., R.C., Norton, W.N., Howard, G.T., 1998. Adherence and characterization of metabolites produced. Applied Environmental
growth of a Bacillus species on an insoluble polyester polyurethane. Microbiology 59, 3695–3700.
International Biodeterioration & Biodegradation 42, 63–73. Caldwell, D.E., Lawrence, J.R., 1986. Growth kinetics of Pseudomonas
Blanchette, R.A., 1995. Biodeterioration of archaeological wood. uorescens microcolonies within the hydrodynamic boundary layers
Biodeterioration Abstract 9, 113–127. of surface microenvironments. Microbial Ecology 12, 299–312.
Bloomÿeld, S.F., Megid, R., 1994. Interaction of iodine with Bacillus Caldwell, D.E., Wolfaaedt, G.M., Korber, D.R., Lawrence, J.R., 1997. Do
subtilis spores and spore forms. Journal of Applied Bacteriology 76, bacterial communities transcend Darwinism? Advances in Microbial
492–499. Ecology 15, 105–191.
Bogan, R.T., Brewer, R.T., 1985. Cellulose esters, organic. In: Callow, M.E., Fletcher, R.L., 1994. The in uence of low surface energy
Encyclopedia of Polymers Science and Engineering, 2nd Edition. materials on bioadhesion—a review. International Biodeterioration &
Wiley, New York, pp. 158–181. Biodegradation 34, 333–348.
Bonet, R., Simon-Pujol, M.D., Congregado, F., 1993. E ects of nutrients Cargill, K.L., Pyle, B.H., McFeters, G.A., 1992. E ects of culture
on exopolysacchaaride production and surface properties of Aeromonas conditions and bioÿlm formation on the iodine susceptibility of
salmonicida. Applied and Environmental Microbiology 59, 2437–2441. Legionella pneumophila. Canadian Journal of Microbiology 38,
Bos, R., van der Mei, H.C., Busscher, H.J., 1999. Physico-chemistry of 423–429.
initial microbial adhesion interactions—its mechanisms and methods e
Chahal, P.S., Chahal, D.S., AndrÃ , G., 1992. Cellulase production proÿle
for study. FEMS Microbiological Reviews 23, 179–230. of Trichoderma reesei on di erent cellulosic substrates at various pH
Bouwer, E.J., 1992. Bioremediation of organic contaminants in the levels. Journal of Fermentation and Bioengineering 74, 126–128.
subsurface. In: Mitchell, R. (Ed.), Environmental Microbiology. Wiley, Characklis, W.G., 1990. Microbial fouling. In: Characklis, W.G., Marshall,
New York, pp. 319–333. K.C. (Eds.), Bioÿlms. Wiley, New York, pp. 523–584.
Brandl, H., Gross, R.A., Lenz, R.W., Fuller, R.C., 1988. Pseudomonas
Chen, X., Stewart, P.S., 1996. Chlorine penetration into artiÿcial bioÿlm
oleovorans as a source of poly(ÿ-hydroxyalkanoates) for potential
is limited by a reaction-di usion interaction. Environmental Science
application as biodegradable polyesters. Applied and Environmental
and Technology 30, 2078–2083.
Microbiology 54, 1977–1982.
Choi, M.H., Yoon, S.C., 1994. Polyester biosynthesis characteristics
Breslin, V.T., 1993. Degradation of starch–plastic composites in a
of Pseudomonas citronellolis grown on various carbon sources,
municipal solid waste landÿll. Journal of Environmental Polymer
including 3-methyl-branched substrates. Applied and Environmental
Degradation 1, 127–141.
Microbiology 60, 3245–3254.
Breslin, V.T., Swanson, R.L., 1993. Deterioration of starch–plastic
Costerton, J.W., Geesey, G.G., Cheng, K.-J., 1978. How bacteria stick.
composite in the environment. Journal of Air Waste Management
Scientiÿc American 238, 86–95.
Association 43, 325–335.
Costerton, J.W., Geesey, G.G., Jones, P.A., 1988. Bacterial bioÿlms
Breznak, J.A., 1984. Activity on surfaces. In: Marshall, K.C. (Ed.),
in relation to internal corrosion monitoring and biocide strategies.
Microbial Adhesion and Aggregation. Dahlem Konferenzen. Springer,
Materials Performance 4, 49–53.
Berlin, pp. 203–221.
Brown, G.A., 1982. Implications of electronic and ionic conductivities of Costerton, J.W., Lewandowski, Z., DeBeer, D., Caldwell, D., Korber,
polyimide ÿlms in integrated circuit fabrication. In: Feit, E.D., Wilkins, D., James, G., 1994. Bioÿlms, the customized microniche. Journal of
C.W. (Eds.), Polymer Materials for Electronic Applications. ACS Bacteriology 176, 2137–2142.
Symposium Series No. 184. American Chemical Society, Washington, Costerton, J.W., Lewandowski, Z., Caldwell, D.E., Korber, D.R.,
DC, pp. 151–169. Lappin-Scott, H.M., 1995. Microbial bioÿlms. Annual Reviews of
Brozel, V.S., Cloete, T.E., 1993. Bacterial resistance to conventional water Microbiology 49, 711–745.
treatment biocides. Biodeterioration Abstracts 7, 387–395. Crabbe, J.R., Campbell, J.R., Thompson, L., Walz, S.L., Scultz, W.W.,
Brune, A., Frenzel, P., Cypionka, H., 2000. Life at the oxic–anoxic 1994. Biodegradation of a colloidal ester-based polyurethane by soil
interface: microbial activities and adaptations. FEMS Microbiological fungi. International Biodeterioration & Biodegradation 33, 103–113.
Reviews 24, 691–710. Cromwick, A.-M., Gross, R.A., 1995. Investigation by NMR of metabolic
Bryers, J.D., 1990. Bioÿlms in biotechnology. In: Characklis, W.G., routes to bacterial -poly(glutamic acid) using 13 C-labelled citrate and
Marshall, K.C. (Eds.), Bioÿlms. Wiley, New York, pp. 733–773. glutamate as media carbon source. Canadian Journal of Microbiology
Bryers, J.D., 1994. Bioÿlms and the technological implications of 41, 902–909.
microbial cell adhesion. Colloidal Surfaces B: Biointerfaces 2, 9–23. Cunningham, A.B., Bouwer, E.J., Characklis, W.G., 1990. Bioÿlms in
Bryers, J.D., Characklis, W.G., 1990. Bioÿlms in water and wastewater porous media. In: Characklis, W.G., Marshall, K.C. (Eds.), Bioÿlms.
treatment. In: Characklis, W.G., Marshall, K.C. (Eds.), Bioÿlms. Wiley, Wiley, New York, pp. 697–732.
New York, pp. 671–696. Cunningham, A.M., Characklis, W.G., Abedeen, F., Crawford, D., 1991.
Buchanan, C.M., Gardner, R.M., Komarek, R.J., 1993. Aerobic In uence of bioÿlm accumulation on porous media hydrodynamics.
biodegradation of cellulose acetate. Journal of Applied Polymer Science Environmental Science and Technology 25, 1305–1311.
47, 1709–1719. Dalton, H.M., Poulsen, L.K., Halasz, P., Angles, M.L., Goodman, A.E.,
Budwill, K., Fedorak, P.M., Page, W.J., 1992. Methanogenic Marshall, K.C., 1994. Substratum-induced morphological changes in a
degradation of poly(3-hydroxyalkanoates). Applied and Environmental marine bacterium and their relevance to bioÿlm structure. Journal of
Microbiology 58, 1398–1401. Bacteriology 176, 6900–6906.
84 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Davey, M.E., O’Toole, G.A., 2000. Microbial bioÿlms: from ecology to Ford, T., Maki, J., Mitchell, R., 1995. Metal-microbe interactions. In:
molecular genetics. Microbiology and Molecular Biology Reviews 64, Gaylarde, C.C., Videla, H.A. (Eds.), Bioextraction and Biodeterioration
47–867. of Metals. Cambridge University Press, New York, pp. 1–23.
Davies, D.G., Parsek, M.R., Pearson, P., Iglewski, B.H., Costerton, J.W., Frazer, A.C., 1994. O-methylation and other transformations of aromatic
Greenberg, E.P., 1998. The involvement of cell-to-cell signals in the compounds by acetogenic bacteria. In: Drake, H.L. (Ed.), Acetogenesis.
development of a bacterial bioÿlm. Science 280, 295–298. Chapman & Hall, New York, pp. 445–483.
Dobbins, J.J., Giammara, B.L., Hanker, J.S., Yates, P.E., DeVries, W.C., Freeman, C., Lock, M.A., 1995. The bioÿlm polysaccharide matrix:
1989. Demonstration of the bacterial–biomaterial interface in implant a bu er against chaging organic substrate supply?. Limnology and
specimens. In: Materials Research Society Symposium Proceedings, Oceanography 40, 273–278.
Vol. 110. Materials Research Society, Philadelphia, Pennsylvania, pp. Frings, J., Schramm, E., Schink, B., 1992. Enzymes involved in
337–348. anaerobic polyethylene glycol degradation by Pelobacter venetianus
Doi, Y., 1990. Microbial Polyesters. VCH Publishers, New York. and Bacteroides Strain PG1. Applied and Environmental Microbiology
Downing, K.M., Ho, C.S., Zabriskie, D.W., 1987. Enzymatic production 58, 2164–2167.
of ethanol from cellulose using soluble cellulose acetate as an Fuchs, D.R., Popall, M., Romich, H., Schmidt, H., 1991. Preservation
intermediate. Biotechnology and Bioengineering 29, 1086–1096. of stained glass windows: new materials and techniques. In: Baer,
Dwyer, D., Tiedje, J.M., 1983. Degradation of ethylene glycol N.S., Sabbioni, C., Sors, A.I. (Eds.), Science, Technology and
and polyethylene glycols by methanogenic consortia. Applied and European Cultural Heritage. Butterworth-Heinemann, Oxford, England,
Environmental Microbiology 46, 185–190. pp. 679–683.
Edwards, D.P., Nevell, T.G., Plunkett, B.A., Ochiltree, B.C., Gamerith, G., Groicher, R., Zeilinger, S., Herzog, P., Kubicek, C.P., 1992.
1994. Resistance to marine fouling of elastomeric coatings of Cellulase-poor xylanases produced by Trichoderma reesei RUT C-30
some poly(dimethylsiloxanes) and poly(dimethyldiphenylsiloanes). on hemicellulose substrates. Applied Microbiology and Biotechnology
International Biodeterioration & Biodegradation 34, 349–359. 38, 315–322.
El-Sayed, A.H.M.M., Mohmoud, W.M., Davis, E.M., Coughlin, Gazenko, O.G., Grigoryev, A.I., Bugrov, S.A., Yegorov, V.V.,
R.W., 1996. Biodegradation of polyurethane coatings by Bogomolov, V.V., Kozlovskaya, I.B., Tarasov, I.K., 1990. Review of
hydrocarbon-degrading bacteria. International Biodeterioration & the major results of medical research during the ight of the second
Biodegradation 37, 69–79. prime crew of the Mir space station. Kosmicheskaya Biologiya i
Ezeonu, I.M., Noble, J.A., Simmons, R.B., Price, D.L., Crow, S.A., Aviakosmicheskaya Medistina 23, 3–11 (in Russian).
Ahearn, D.G., 1994a. E ect of relative humidity on fungal colonization Geesey, G.G., White, D.C., 1990. Determination of bacterial growth and
of ÿberglass insulation. Applied and Environmental Microbiology 60, activity at solid–liquid interfaces. Annual Reviews of Microbiology
2149–2151. 44, 579–602.
Ezeonu, I.M., Price, D.L., Simmons, R.B., Crow, S.A., Ahearn, D.G., Geesey, G.G., Gills, R.J., Avci, R., Daly, D., Hamilton, M., Shope,
1994b. Fungal production of volatiles during growth on ÿberglass. P., Harkon, G., 1996. The in uence of surface features on bacterial
Applied and Environmental Microbiology 60, 4172–4173. colonization and subsequent substratum chemical changed of 316L
Fabbri, A.A., Ricelli, A., Brasini, S., Fanelli, C., 1997. E ect of di erent stainless steel. Corrosion Science 38, 73–95.
antifungals on the control of paper biodeterioration caused by fungi. Gehrke, T., Telegdi, J., Thierry, D., Sand, W., 1998. Importance of
International Biodeterioration & Biodegradation 39, 61–65. extracellular polymeric substances from Thiobacillus ferrooxidants for
Fan, Y., Cheng, S.P., Gu, J.-D., 2001. Degradation of phthalic acid and bioleaching. Applied and Environmental Microbiology 64, 2743–2747.
dimethyl phthalate ester by an aerobic enrichment of microorganisms. Gillatt, J., 1990. The biodeterioration of polymer emulsions and its
In: Sun, D.D., Wilson, F. (Eds.), IWA Asia Environmental Technology prevention with biocides. International Biodeterioration 26, 205–216.
2001. Nanyang University of Technology, Singapore, pp. 547–554. Gillis, R.J., Gillis, J.R., 1996. A comparative study of bacterial attachment
Fenchel, T., Finlay, B.J., 1995. Ecology and Evolution in Anoxic Worlds. to high-purity water system surfaces. Ultrapure Water 9, 27–36.
Oxford University Press, New York. Gilmore, D.F., Antoun, S., Lenz, R.W., Goodwin, S., Austin, R., Fuller,
Filip, Z., 1978. Decomposition of polyurethane in a garbage landÿll R.C., 1992. The fate of biodegradable plastics in municipal leaf
leakage water and by soil microorganisms. European Journal of Applied compost. Journal of Industrial Microbiology 10, 199–206.
Microbiology 5, 225–231. Gilmore, D.F., Antoun, S., Lenz, R.W., Fuller, R.C., 1993. Degradation
Flemming, H.-C., Schaule, G., McDonogh, R., Ridgway, H.F., 1994. of poly(ÿ-hydroxyalkanoates) and polyoleÿn blends in a municipal
E ects and extent of bioÿlm accumulation in membrane systems. In: wastewater treatment facility. Journal of Environmental Polymer
Geesey, G.G., Lewandowski, Z., Flemming, H.-C. (Eds.), Biofouling Degradation 1, 269–274.
and Biocorrosion in Industrial Water Systems. Lewis Publishers, Boca Gross, R.A., Gu, J.-D., Eberiel, D., Nelson, M., McCarthy, S.P., 1993.
Raton, FL, pp. 63–89. Cellulose acetate biodegradability in simulated aerobic composting and
Fletcher, M., 1996. Bacterial attachment in aquatic environments: a anaerobic bioreactors as well as by a bacterial isolate derived from
diversity of surfaces and adhesion strategies. In: Fletcher, M. (Ed.), compost. In: Kaplan, D., Thomas, E., Ching, C. (Eds.), Fundamentals
Bacterial Adhesion: Molecular and Ecological Diversity. Wiley-Liss, of Biodegradable Materials and Packaging. Technomic Publishing Co,
New York, pp. 1–24. Lancaster, Pennsylvania, pp. 257–279.
Fletcher, M., Loeb, G.I., 1979. In uence of substratum characteristics on Gross, R.A., Gu, J.-D., Eberiel, D., McCarthy, S.P., 1995. Laboratory
the attachment of a marine Pseudomonad to solid surfaces. Applied scale composting test methods to determine polymer degradability:
and Environmental Microbiology 37, 67–72. model studies on cellulose acetate. In: Albertson, A., Huang, S. (Eds.),
Florian, M.-L.E., 1996. The role of the conidia of fungi in fox spots. Degradable Polymers, Recycling and Plastics Waste Management.
Studies in Conservation 41, 65–75. Marcel Dekker, New York, pp. 21–36.
Ford, T.E., 1993. The microbial ecology of water distribution and outfall Gu, J.-D., 2001. Degradability of N-heterocyclic aromatic compounds by
systems. In: Ford, T.E. (Ed.), Aquatic Microbiology: An Ecological anaerobic microorganisms from marine sediments and immobilization
Approach. Blackwell, Boston, MA, pp. 455–482. on surfaces. Contaminated Sediment and Water. August (International
Ford, T., Sacco, E., Black, J., Kelley, T., Goodacre, R., Berkley, Issue), 57–59.
R.C.W., Mitchell, R., 1991. Characterization of exopolymers of aquatic Gu, J.-D., Berry, D.F., 1991. Degradation of substituted indoles
bacteria by pyrolysis-mass spectroscopy. Applied and Environmental by an indole-degrading methanogenic consortium. Applied and
Microbiology 57, 1595–1601. Environmental Microbiology 57, 2622–2627.
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 85
Gu, J.-D., Berry, D.F., 1992. Metabolism of 3-methylindole by a Gu, J.-D., Ford, T.E., Thorp, K.E.G., Mitchell, R., 1996a. Microbial
methanogenic consortium. Applied and Environmental Microbiology growth on ÿber reinforced composite materials. International
58, 2667–2669. Biodeterioration & Degradation 39, 197–204.
Gu, J.-D., Cheung, K.H., 2001. Phenotypic expression of Vogesella Gu, J.-D., Ford, T.E., Mitchell, R., 1996b. Susceptibility of electronic
indigofera upon exposure to hexavalent chromium, Cr 6+ . World insulating polyimides to microbial degradation. Journal of Applied
Journal of Microbiology & Biotechnology 17, 475–480. Polymer Science 62, 1029–1034.
Gu, J.-D., Mitchell, R., 1995. Microbiological in uenced corrosion of Gu, J.-D., Lu, C., Thorp, K., Crasto, A., Mitchell, R., 1996c. Susceptibility
metal, degradationa and deterioration of polymeric materials of space of polymeric coatings to microbial degradation. Corrosion/96, Paper
application. Chinese Journal of Materials Research 9 (Suppl.), 473– No. 275, NACE International, Houston, Texas.
489 (in English). Gu, J.-D., Ford, T.E., Berke, N.S., Mitchell, R., 1996d. Fungal
Gu, J.-D., Mitchell, R. 2001. Biodeterioration. In: Dworkin, M., Falkow, degradation of concrete. In: Sand, W. (Ed.), Biodeterioration
S., Rosenberg, E., Schleifer, K.-H., Stackebrandt, E. (Eds.), The and Biodegradation, DECHEMA Monographs, Vol. 133. VCH
Prokaryotes: An Evolving Electronic Resource for the Microbiological Verlagsgesellschaft, Frankfurt, Germany, pp. 135 –142.
Community. (3rd ed.) Springer-Verlag, New York.
Gu, J.-D., Thorp, K., Crasto, A., Mitchell, R., 1996e. Microbiological
Gu, J.-D., Berry, D.F., Taraban, R.H., Martens, D.C., Walker, Jr., H.L.,
degradation of ÿber-reinforced polymeric composites. In: The
Edmonds, W.J., 1992a. Biodegradability of atrazine, cyanazine, and
Electrochemical Society Spring Meeting, May 5 –10, Los Angeles. The
dicamba in wetland soils. Virginia Water Resource Research Center,
Electrochemical Society, Pennington, NJ, pp. 143–144.
Bull. No. 172, Blacksburg, Virginia.
Gu, J.-D., Lu, C., Thorp, K., Crasto, A., Mitchell, R., 1997a.
Gu, J.-D., Gada, M., Kharas, G., Eberiel, D., McCarty, S.P., Gross,
Fungal degradation of ÿber-reinforced composite materials. Materials
R.A., 1992b. Degradability of cellulose acetate (1.7 and 2.5, d.s.) and
Performance 36, 37–42.
poly(lactide) in simulated composting bioreactors. Polymer Materials:
Science and Engineering 67, 351–352. Gu, J.-D., Lu, C., Thorp, K., Crasto, A., Mitchell, R., 1997b.
Gu, J.-D., McCarty, S.P., Smith, G.P., Eberiel, D., Gross, R.A., 1992c. Fiber-reinforced polymeric composite materials are susceptible
Degradability of cellulose aceteate (1.7, d.s.) and cellophane in to microbial degradation. Journal of Industrial Microbiology &
anaerobic bioreactors. Polymer Materials: Science and Engineering 67, Biotechnology 18, 364–369.
230–231. Gu, J.-D., Maki, J.S., Mitchell, R., 1997c. Microbial bioÿlms and their
Gu, J.-D., Coulter, S., Eberiel, D., McCarthy, S.P., Gross, R.A., 1993a. A role in the indiction and inhibition of invertebrate settlement. In: D’Itri,
respirometric method to measure mineralization of polymeric materials F.M. (Ed.), Zebra Mussels and Aquatic Nuisance Species. Ann Arbor
in a matured compost environment. Journal of Environmental Polymer Press, Chelsea, Michigan, pp. 343–357.
Degradation 1, 293–299. Gu, J.-D., Mitton, D.B., Ford, T.E., Mitchell, R., 1998a. Microbial
Gu, J.-D., Eberiel, D.T., McCarthy, S.P., Gross, R.A., 1993b. degradation of polymeric coatings measured by electrochemical
Cellulose acetate biodegradability upon exposure to simulated aerobic impedance spectroscopy. Biodegradation 9, 35–39.
composting and anaerobic bioreactor environments. Journal of Gu, J.-D., Roman, M., Esselman, T., Mitchell, R., 1998b. The role of
Environmental Polymer Degradation 1, 143–153. microbial bioÿlms in deterioration of space station candidate materials.
Gu, J.-D., Eberiel, D., McCarthy, S.P., Gross, R.A., 1993c. International Biodeterioration & Biodegradation 41, 25–33.
Degradation and mineralization of cellulose acetate in simulated Gu, J.-D., Ford, T.E., Berke, N.S., Mitchell, R., 1998c. Biodeterioration
thermophilic composting environment. Journal of Environmental of concrete by the fungus Fusarium. International Biodeterioration &
Polymer Degradation 1, 281–291. Biodegradation 41, 101–109.
Gu, J.-D., Ford, T.E., Thorp, K.E.G., Mitchell, R., 1994a. Microbial Gu, J.-D., Ford, T.E., Mitchell, R., 2000a. Microbial corrosion of metals.
degradation of polymeric materials. In: Naguy, T. (Ed.), Proceedings In: Revie, W. (Ed.), The Uhlig Corrosion Handbook, 2nd Edition.
of the Tri-Service Conference on Corrosion, June 21–23, Orlando, Wiley, New York, pp. 915–927.
Florida. U.S. Government Printing House, Washington, DC, Gu, J.-D., Ford, T.E., Mitton, D.B., Mitchell, R., 2000b. Microbial
pp. 291–302. degradation and deterioration of polymeric materials. In: Revie, W.
Gu, J.-D., Yang, S., Welton, R., Eberiel, D., McCarthy, S.P., Gross, (Ed.), The Uhlig Corrosion Handbook, 2nd Edition. Wiley, New York,
R.A., 1994b. E ects of environmental parameters on the degradability pp. 439–460.
of polymer ÿlms in laboratory-scale composting reactors. Journal of Gu, J.-D., Ford, T.E., Mitchell, R., 2000c. Microbial corrosion of concrete.
Environmental Polymer Degradation 2, 129–135. In: Revie, W. (Ed.), The Uhlig Corrosion Handbook, 2nd Edition.
Gu, J.-D., Ford, T.E., Mitton, B., Mitchell, R., 1995a. Microbial Wiley, New York, pp. 477–491.
degradation of complex polymeric materials used as insulation in
Gu, J.-D., Ford, T.E., Mitchell, R., 2000d. Microbial degradation of
electronic packaging materials. Corrosion/95, Paper No. 202, National
materials: general processes. In: Revie, W. (Ed.), The Uhlig Corrosion
Association of Corrosion Engineers, Houston, Texas.
Handbook, 2nd Edition. Wiley, New York, pp. 349–365.
Gu, J.-D., Ford, T.E., Thorp, K.E.G., Mitchell, R., 1995b. Microbial
biodeterioration of ÿber reinforced composite materials. In: Angell, Gu, J.-D., Gu, J.-G., Shi, H.C., Li, X.Y., 2000e. Simulating anaerobic
P., Borenstein, S.W., Buchanan, R.A., Dexter, S.C., Dowling, N.J.E., landÿll conditions in bioreactors and testing polymer degradability
Little, B.J., Lundin, C.D., McNeil, M.B., Pope, D.H., Tatnall, R.E., using poly(ÿ-hydroxybutyrate-co-16% valerate) and cellulose acetates
White, D.C., Zigenfuss, H.G. (Eds.), International Conference on (DS 1.7 and 2.5). Water Science and Technology, in press.
Microbial In uenced Corrosion. NACE International, Houston, Texas, Gu, J.-D., Belay, B., Mitchell, R., 2001a. Protection of catheter surfaces
pp. 25/1–7. from adhesion of Pseudomonas aeruginosa by a combination of silver
Gu, J.-D., Ford, T.E., Thorp, K.E.G., Mitchell, R., 1995c. Microbial ions and lectins. World Journal of Microbiology & Biotechnology 17,
deterioration of ÿber reinforced polymeric materials. In: Scully, 173–179.
J. (Ed.), Corrosion/95, Research in Progress Symposium. NACE Gu. J.-D., Cheng, S., Gu, J.-G. 2001b. Degradation of the herbicide
International, Houston, Texas, pp. 16–17. dicamba under strictly anaerobic conditions. Chinese Journal of
Gu, J.-D., Ford, T.E., Thorp, K.E.G., Mitchell, R., 1995d. E ects of Environmental Science 22, 111–113. (in Chinese).
microorganisms on stability of ÿber reinforced polymeric composites. Gu, J.-D., Fan, Y., Shi, H., 2001c. Degradation mechanisms of indolic
Second International Conference on Composites Engineering, August compounds under methanogenic conditions. In: Sun, D.D., Wilson,
21–24, University of New Orleans, New Orleans, Louisiana, F. (Eds.), IWA Asia Environmental Technology 2001, October 30 –
pp. 279 –280. November 3, 2001, Singapore, pp. 296 –302.
86 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Guezennec, J., Ortega-Morales, O., Raguenes, G., Geesey, G., 1998. Karlsson, S., Ljungquist, O., Albertsson, A.-C., 1988. Biodegradation of
Bacterial colonization of artiÿcial substrate in the vicinity of deep-sea polyethylene and the in uence of surfactants. Polymer Degradability
hydrothermal vents. FEMS Microbiology Ecology 26, 89–99. and Stability 21, 237–250.
Gujer, W., Zehnder, A.J.B., 1983. Conversion processes in anaerobic Kawai, F., 1987. The biochemistry of degradation of polyethers. CRC
digestion. Water Science and Technology 15, 127–167. Critical Reviews in Biotechnology 6, 273–307.
Gunjala, K.R., Sul ita, J.M., 1993. Environmental factors in uencing Kawai, F., 2002. Microbial degradation of polyethers. Applied
methanogenesis from refuse in landÿll samples. Environmental Science Microbiology and Biotechnology 58, 30–38.
and Technology 27, 1176–1181. Kawai, F., Moriya, F., 1991. Bacterial assimilation of polytetramethylene
Hahn, P.O., Rublo , G.W., Bartha, J.W., Legoues, F., Tromp, R., Ho, P.S., glycol. Journal of Fermentation and Bioengineering 71, 1–5.
1985. Chemical interactions at metal–polymer interfaces. In: Materials Kawai, F., Yamanaka, H., 1986. Biodegradation of polyethylene glycol
Research Society Symposium Proceedings, Vol. 40. Materials Research by symbiotic mixed culture (Obligate mutulism). Archives of
Society, Pittsburgh, Pennsylvania, pp. 251–263. Microbiology 146, 125–129.
Hamilton, J.D., Reinert, K.H., Hogan, J.V., Lord, W.V., 1995. Polymers Kawai, F., Yamanaka, H., 1989. Inducible or constitutive polyethylene
as solid waste in municipal landÿlls. Journal of Air Waste Management glycol dehydrogenase involved in the aerobic metabolism of
Association 43, 247–251. polyethylene glycol. Journal of Fermentation and Bioengineering 67,
Hass, H., Herfurth, E., Sto er, G., Redl, B., 1992. Puriÿcation, 300–302.
characterization and partial amino acid sequences of a xylanase Keevil, C.W., Mackerness, C.W., 1990. Biocide treatment of bioÿlms.
produced by Penicillium chrysogenum. Biochimic et Biophysica Acta International Biodeterioration 26, 169–179.
1117, 279–286. Kelley, K., Ishino, Y., Ishida, H., 1987. Fourier transform IR re ection
Heisey, R.M., Papadatos, S., 1995. Isolation of microorganisms able techniques for characterization of polyimide ÿlms on copper substrates.
to metabolize puriÿed natural rubber. Applied and Environmental Thin Solid Films 154, 271–279.
Microbiology 61, 3092–3097. Kelley-Wintenberg, K., Montie, T.C., 1994. Chemotaxis to oligopeptides
Hespell, R.B., O’Bryan-Shah, P.J., 1988. Esterase activities in Butyrivibrio by Pseudomonas aeruginosa. Applied and Environmental
ÿbrisolvens strains. Applied and Environmental Microbiology 54, Microbiology 60, 363–367.
Kemnitzer, J.E., McCarthy, S.P., Gross, R.A., 1992. Poly(ÿ-hydroxy-
butyrate) stereoisomers: a model study of the e ects of stereochemical
Holmes, P.A., Wright, L.F., Colins, S.H., 1985. ÿ-hydroxybutyrate
and morphological variables on polymer biological degradability.
polymers. European Patent Application EP 52, 459.
Macromolecules 22, 5927–5934.
Hou, B., 1999. Haiyang Fushi Huanjing Lilun Jiqi Yingyong (Marine
Kemnitzer, J.E., McCarthy, S.P., Gross, R.A., 1993. Syndiospeciÿc
and environmental corrosion: theory and applications). China Science
ring-opening polymerization of ÿ-butyrolactone to form predominantly
Press, Beijing, pp. 107–131.
syndiotactic poly(ÿ-hydroxybutyrate) using Tin (IV) catalysts.
Huang, C.-T., James, G., Pitt, W.G., Stewart, P.S., 1996. E ects of
Macromolecules 23, 6143–6150.
ultrasonic treatment on the e cacy of gentamicin against established
Kim, O., Gross, R.A., Rutherford, D.R., 1995. Bioengineering
Pseudomonas aeruginosa bioÿlms. Colloidal Surfaces B: Biointerfaces
of poly(ÿ-hydroxyalkanoates) for advanced material applications:
incorporation of cyano and nitrophenoxy side chain substituents.
Imam, S.H., Gould, J.M., 1990. Adhesion of an amylolytic Arthrobacter
Canadian Journal of Microbiology 41 (Suppl.), 32–43.
sp. to starch-containing plastic ÿlms. Applied and Environmental
King, B., Eggins, H.O.W, 1972. Some observations on decay mechanisms
Microbiology 56, 872–876.
of microfungi deteriorating wood. In: Walters, A.H., Hueck-van der
Imam, S.H., Gould, J.M., Gordon, S.H., Kinney, M.P., Ramsey, A.M.,
Plas, E.H. (Eds.), Biodeterioration of Materials. Halsted Press Div,
Tosteson, T.R., 1992. Fate of starch-containing plastic ÿlms exposed
Wiley, New York, pp. 145–151.
in aquatic habitats. Current Microbiology 25, 1–8. Knyazev, V.M., Korolkov, V.I., Viktorov, A.N., Pozharskiy, G.O.,
Imam, S.H., Gordon, S.H., Shogren, R.L., Tosteson, T.R., Govind, N.S., Petrova, L.N., Gorshkov, V.P., 1986. Sanitary and microbiological
Greene, R.V., 1999. Degradation of starch-poly(ÿ-hydroxybutyrate- aspects of closed environment occupied by people and animals.
co-ÿ-hydroxyvalerate) bioplastic in tropical coastal waters. Applied Kosmicheskaya Biologiya i Aviakosmicheskaya Medistina 20, 80–82
and Environmental Microbiology 65, 431–437. (in Russian).
Jensen, R.J., 1987. Polyimides as interlayer dielectrics for Koenig, D.W., Mishra, S.K., Pierson, D.L., 1995. Removal of
high-performance interconnections of integrated circuits. In: Bouwden, Burkholderia cepacia bioÿlms with oxidants. Biofouling 9, 51–62.
M.J., Turner, S.R. (Eds.), Polymers for High Technology—Electronics Kohler, H.-P.E., Nickel, K., Zipper, C., 2000. E ect of chirality on the
and Photonics. ACS Symposium Series No. 346. American Chemical microbial degradation and the environmental fate of chiral pollutants.
Society, Washington, DC, pp. 466–483. In: Schink, B. (Ed.), Advances in Microbial Ecology, Vol. 16. Kluwer
John, M.E., Keller, G., 1996. Metabolic pathway engineering in cotton: Academic/Plenum Publishers, New York, pp. 201–231.
biosynthesis of polyhydroxybutyrate in ÿber cells. Proceedings of Konhauser, K.O., Schultze-Lam, S., Ferris, F.G., Fyfe, W.S., Longsta e,
National Academy of Science (USA) 93, 768–773. F.J., Beveridge, T.J., 1994. Mineral precipitation by epilithic bioÿlms
Jones-Meehan, J., Vasanth, K.L., Conrad, R.K., Fernandez, M., Little, B.J., in the Speed River, Ontario, Canada. Applied and Environmental
Ray, R.I., 1994a. Corrosion resistance of several conductive caulks and Microbiology 60, 549–553.
sealants from marine ÿeld tests and laboratory studies with marine, Korber, D.R., Lawrence, J.R., Sutton, B., Caldwell, D.E., 1989. E ect of
mixed communities containing sulfate-reducing bacteria (SRB). In: laminar ow velocity on the kinetics of surface recolonization by Mot +
Kearns, J.R., Little, B.J. (Eds.), Microbiologically In uenced Corrosion and Mot − Pseudomonas uorescens. Microbial Ecology 18, 1–9.
Testing. ASTM STP 1232. American Society for Testing and Materials, Kormelink, F.J.M., Voragen, J., 1993. Degradation of di erent
Philadelphia, Pennsylvania, pp. 217–233. [(glucurono)arabino]xylans by a combination of puriÿed xylan–
Jones-Meehan, J., Walch, M., Little, B.J., Ray, R.I., Mansfeld, F.B., 1994b. degrading enzymes. Applied Microbiology and Biotechnology 38,
E ect of mixed sulfate-reducing bacterial communities on coatings. In: 688–695.
Geesey, G.G., Lewandowski, Z., Flemming, H.-C. (Eds.), Biofouling Krieg, N.R., Holt, J.G., 1984. Bergey’s Manual of Systematic
and Biocorrosion in Industrial Water Systems. Lewis Publishers, Boca Bacteriology, Vol. 1. Williams and Wilkins, Baltimore, MD.
Raton, FL, pp. 107–135. Lai, J.H., 1989. Polymers for Electronic Applications. CRC Press, Boca
Kaplan, D.L., Lombardi, S.J., Muller, W.S., Fossey, S.A., 1991. Silk. Ralton, Florida.
In: Byrom, D. (Ed.), Biomaterials: Novel Materials from Biological Lappin-Scott, H., Costerton, J.W., Marrie, T.J., 1992. Bioÿlms and
Sources. Macmillan Publishers, Great Britain, pp. 1–53. biofouling. Encyclopedia of Microbiology 1, 277–284.
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 87
Lauwers, A.M., Heinen, W., 1974. Biodegradation and utilization of silica Luthi, E., Jasmat, N.B., Bergquist, P.L., 1990a. Over-production of
and quartz. Archives of Microbiology 95, 67–78. an acetylxylan esterase from the extreme thermophile “Caldocellum
Lawrence, J.R., Delaquis, P.J., Korber, D.R., Caldwell, D.E., 1987. saccharolyticum” in Escherichia coli. Applied Microbiology and
Behavior of Pseudomonas uorescens within the hydrodynamic Biotechnology 34, 214–219.
boundary layers of surface microenvironments. Microbial Ecology 14, Luthi, E., Love, D.R., McAnulty, J., Wallace, C., Caughey, P.A.,
1–14. Saul, D., Bergquist, P.L., 1990b. Cloning, sequence analysis,
Lee, S.F., Forsberg, C.W., Gibbins, L.N., 1985. Xylanolytic activity of and expression of genes encoding xylan-degrading enzymes from
Clostridium acetobutylicum. Applied and Environmental Microbiology the thermophile “Caldocellum saccharolyticum”. Applied and
50, 1068–1076. Environmental Microbiology 56, 1017–1024.
Lee, S.F., Forsberg, C.W., Rattray, J.B., 1987a. Puriÿcation Lynch, J.L., Edyvean, R.G.J., 1988. Biofouling in oilÿeld water systems—
and characterization of two endoxylanases from Clostridium a review. Biofouling 1, 147–162.
acetobutylicum. ATCC 824. Applied and Environmental Microbiology MacDonald, M.J., Hartley, D.L., Speedie, M.K., 1985. Location of
53, 644–650. cellulolytic enzyme activity in the marine fungus Trichocladium
Lee, H., To, R.J.B., Latta, R.K., Biely, P., Schneider, H., 1987b. Some achrasporum. Canadian Journal of Microbiology 31, 145–148.
properties of extracellular acetylxylan esterase produced by the yeast MacKenzie, C.R., Bilous, D., Schneider, H., Johnsom, K.G., 1987.
Rhodotorula mucilaginosa. Applied and Environmental Microbiology Induction of cellulolytic and xylanolytic enzyme systems in
53, 2831–2834. Streptomyces spp. Applied and Environmental Microbiology 53,
Lee, Y.-E., Lowe, S.E., Zeikus, J.G., 1993. Regulation and characterization 2853–2859.
of xylanolytic enzymes of Thermoanaerobacterium saccharolyticum Madigan, M.T., Martinko, J.M., Parker, J., 2000. Brock Biology of
B6A-RI. Applied and Environmental Microbiology 59, 763–771. Microorganisms, 9th Edition. Prentice-Hall, Upper Saddle River, NJ.
Lemaire, J., Dabin, P., Arnaud, R., 1992. Mechanisms of abiotic Maki, J.S., Rittschof, D., Samuelsson, M.-O., Szewyk, U., Yule, A.B.,
degradation of synthetic polymers. In: Vert, M., Feijen, J., Albertsson, Kjelleberg, S., Costlow, J.D., Mitchell, R., 1990. E ect of marine
A., Scott, G., Chiellini, E. (Eds.), Biodegradable Polymers and Plastics. bacteria and their exopolymers on the attachment of barnacle cypris
Royal Society of Chemistry, Cambridge, UK, pp. 30–39. larvae. Bulletin of Marine Science 46, 499–511.
Lemoigne, M., 1926. Produits de deshydration et de polymerisation de Mansfeld, F., 1994. E ectiveness of ion vapor-deposited aluminum as a
l’acide ÿ-oxybutyric. Bulletin dela Societe deli Chimie Biologique primer for epoxy and urethane topcoats. Corrosion 50, 609–612.
(Paris) 8, 770–782. Mansfeld, F., 1995. Use of electrochemical impedance spectroscopy
Lewandowski, Z., Stoodley, P., Altobelli, S., 1995. Experimental and for the study of corrosion by polymer coatings. Journal of Applied
conceptual studies on mass transport in bioÿlms. Water Science and Electrochemistry 25, 187–202.
Technology 31, 153–162. Marshall, K.C., 1976. Interfaces in Microbial Ecology. Harvard University
Leyden, R.N., Basiulis, D.I., 1989. Adhesion and electrical insulation Press, Cambridge, MA.
of thin polymeric coatings under saline exposure. In: Hanker, J.S., Marshall, K.C., 1980. Adsorption of microorganisms to soils and
Giammara, B.L. (Eds.), Biomedical Materials and Devices, Material sediments. In: Bitton, G., Marshall, K.C. (Eds.), Adsorption of
Research Society Symposium Proceedings, Vol. 10. Materials Research Microorganisms to Surfaces. Wiley, New York, pp. 317–329.
Society, Pittsburgh, Pennsylvania, pp. 627–633. Marshall, K.C., 1992. Bioÿlms: an overview of bacterial adhesion, activity,
L’Hostis, E., CompÂ re, C., Festy, D., Tribollet, B., Deslouis, C., 1997.
e and control at surfaces. ASM (American Society for Microbiology)
Characterization of bioÿlms formed on gold in natural seawater by News 58, 202–207.
oxygen di usion analysis. Corrosion 53, 4–10. Marshall, K.C., Stout, R., Mitchell, R., 1971. Mechanism of the initial
Li, D., Ma, Y., Flanagan, W.F., Lichter, B.D., Wikswo Jr., J.P., events in the sorption of marine bacteria to surfaces. Journal of General
1997. Detection of hidden corrosion of aircraft aluminum alloy by Microbiology 68, 337–348.
magnetometry using a superconducting quantum interference device. Martrhamuthu, S., Rajagopal, G., Sathianarayannan, S., Eashwar, M.,
Corrosion 53, 93–98. Balakrishnan, K., 1995. A photoelectrochemical approach to the
Liken, G.E., 1981. Some Perspectives of the Major Biogeochemical ennoblement process: proposal of an adsorbed inhibitor theory.
Cycles. Scope 17. Wiley, New York. Biofouling 8, 223–232.
Linton, J.D., Ash, S.G., Huybrechts, L., 1991. Microbial polysaccharides. a
Mas-CastellÂ , J., Urmeneta, J., Lafuente, R., Navarrete, A., Guerrero,
In: Byrom, D. (Ed.), Biomaterials: Novel Materials from Biological R., 1995. Biodegradation of poly-ÿ-hydroxyalkanoates in anaerobic
Sources. Macmillan Publishers, Great Britain, pp. 215–261. sediments. International Biodeterioration & Biodegradation 35,
Little, B.J., Wagner, P., Maki, J.S., Mitchell, R., 1986. Factors in uencing 155–174.
the adhesion of microorganisms to surfaces. Journal of Adhesion 20, Matamala, G., Smeltzer, W., Droguett, G., 1994. Use of tannin
187–210. anticorrosive reaction primer to improve traditional coating systems.
Little, B., Wagner, P., Characklis, W.G., Lee, W., 1990. Microbial Corrosion 4, 270–275.
corrosion. In: Characklis, W.G., Marshall, K.C. (Eds.), Bioÿlms. Wiley, McCain, J.W., Mirocha, C.J., 1995. Screening computer diskettes
New York, pp. 635–670. and other magnetic media for susceptibility to fungal colonization.
Liu, X., Roe, F., Jesaitis, A., Lewandoski, Z., 1998. Resistance of bioÿlms International Biodeterioration & Biodegradation 33, 255–268.
to the catalase inhibitor 3-amino-1,2,4-triazole. Biotechnology and McFeters, G.A., 1991. Disinfection susceptibility of waterborne
Bioengineering 59, 156–162. Pseudomonads and Legionellae under simulated space vehicle
Lovley, D.R., 1991. Dissimilatory Fe(III) and Mn(IV) reduction. conditions. SAE Technical Paper 911404, Intersociety Conference on
Microbiological Reviews 55, 259–287. Environmental Systems, San Francisco.
Lu, R., Liu, Q., Xiao, C., Bai, S., Chen, H., Wang, F., 1984. Study McFeters, G.A., Yu, F.P., Pyle, B.H., Stewart, P.S., 1995. Physiological
on microbiocidal e ciency of chlorine dioxide for fouling harmful methods to study bioÿlm disinfection. Journal of Industrial
microbes in desalting water systems. Acta Microbiologia Sinica 24, Microbiology 15, 333–338.
243–249. McLean, R.J.C., Nickel, J.C., Olson, M.E., 1995. Bioÿlm associated
Lu, R., Liu, Q., Zhang, Y., Xiao, C., 1989. Studies on harmful microbes in urinary tract infections. In: Lappin-Scott, H.M., Costerton, J.W. (Eds.),
recirculating cooling water system of oil reÿnery. Acta Microbiologia Microbial Bioÿlms. Cambridge university Press, Cambridge, UK, pp.
Sinica 29, 204–215. 261–273.
Lusty, C.J., Doudoro , M., 1966. Poly-ÿ-hydroxybutyrate depolymerases McLean, R.J.C., Whiteley, M., Stickler, D.J., Fuqua, W.C., 1997.
of Pseudomonas lemoignei. Proceedings of National Academy of Evidence of autoinducer activity in naturally occurring bioÿlms. FEMS
Science (USA) 56, 960–965. Microbiology Letters 154, 259–263.
88 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Mergaert, J., Webb, A., Anderson, C., Wouters, A., Swings, Nefedov, Y., Novikova, N.D., Surovezhin, I.N., 1988. Products of
J., 1993. Microbial degradation of poly(3-hydroxybutyrate) and biodegradation of polymers as a factor in the possible pollution of
poly(3-hydroxybutyrate-co-3-hydroxyvalerate) in soils. Applied and the air of thermetically sealed environments with toxic substances.
Environmental Microbiology 59, 3233–3238. Kosmicheskaya Biologiya i Aviakosmicheskaya Medistina 22, 67–71
Mersiosky, I., 2002. Long-term fate of PVC products and their additives (in Russian).
in landÿlls. Progress in Polymer Science 27, 2227–2277. Neu, T., 1996. Signiÿcance of bacterial surface-active compounds in
Meshkov, D., 1994. The in uence of space ight conditions on interaction of bacteria with interfaces. Microbiological Reviews 60,
sensitization of men to bacterial and chemical allergens. 45th 151–166.
Congress of the International Astronautical Confederation Congress, Novikova, N.D., Zaloguyev, S.N., 1985. Formation of volatile
IAF/IAA-94-G.1.125, Jerusalem, Isreal. substances during polymer destruction by Pseudomonas aeruginosa.
Mills, A.L., Powelson, D.K., 1996. Bacterial interactions with surfaces Kosmicheskaya Biologiya i Aviakosmicheskaya Medistina 19, 74–76
in soils. In: Fletcher, M. (Ed.), Bacterial Adhesion: Molecular and (in Russian).
Ecological Diversity. Wiley-Liss, New York, pp. 25 –57. Novikova, N.D., Orlova, M.I., Dyachenko, M.B., 1986. Reproductive
Milstein, O., Gersonde, R., Huttermann, A., Chen, M.-J., Meister, J.J., capacity of micro ora on polymers used in sealed environments.
1992. Fungal biodegradation of lignopolystyrene graft copolymers. Kosmicheskaya Biologiya i Aviakosmicheskaya Medistina 20, 71–73
Applied and Environmental Microbiology 58, 3225–3232. (in Russian).
Mitchell, R., Gu, J.-D., Roman, M., Soulkup, S., 1996. Hazards NRC (National Research Council), 1987. Agenda for Advancing
to space missions from microbial bioÿlms. In: Sand, W. (Ed.), Electrochemical Corrosion Science and Technology. Publication
Biodeterioration and Biodegradation, DECHEMA Monographs, Vol. NMAB438-2, National Academy Press, Washington, DC.
133. VCH Verlagsgesellschaft, Frankfurt, Germany, pp. 3–16. Odian, G., 1991. Principles of Polymerization, 3rd Edition. Wiley,
Mittelman, M.W., 1995. Bioÿlm development in puriÿed water systems. New York.
In: Lappin-Scott, H.M., Costerton, J.W. (Eds.), Microbial Bioÿlms. Osswald, P., Courtes, R., Bauda, P., Block, J.C., Bryers, J.D., Sunde,
Cambridge University Press, Cambridge, UK, pp. 133–147. E., 1995. Xenobiotic biodegradation test using attached bacteria
Mittelman, M.W., 1996. Adhesion to biomaterials. In: Fletcher, M. (Ed.), in synthetic seawater. Ecotoxicology and Environmental Safety 31,
Bacterial Adhesion: Molecular and Ecological Diversity. Wiley-Liss, 211–217.
New York, pp. 89 –127. O’Toole, G., Kaplan, H.B., Kolter, R., 2000. Bioÿlm formation as
Mitton, B., Ford, T.E., LaPointe, E., Mitchell, R., 1993. Biodegradation of microbial development. Annual Review of Microbiology 54, 49–79.
complex polymeric materials. Corrosion/93, Paper No. 296, National Padival, N.A., Weiss, J.S., Arnold, R.G., 1995. Control of Thiobacillus by
Association of Corrosion Engineers, Houston, Texas. means of microbial competition: implications for corrosion of concrete
Mitton, D.B., Latanison, R.M., Bellucci, F., 1996. The e ects of post-cure sewers. Water Environmental Research 67, 201–205.
annealing on the protective properties of polyimides on chromium Parikh, M., Gross, R.A., McCarthy, S.P., 1993. The e ect of crystalline
substrates. Journal of Electrochemical Society 143, 3307–3316. morphology on enzymatic degradation kinetics. In: Kaplan, D.,
Mitton, D.B., Toshima, S., Latanison, R.M., Bellucci, F., Ford, T.E., Gu, Thomas, E., Ching, C. (Eds.), Fundamentals of Biodegradable
J.-D., Mitchell, R., 1998. Biodegradation of polymer-coated metallic Materials and Packaging. Technomic Publishing Co, Lancaster,
substrates. In: Bierwagen, G.P. (Ed.), Organic Coatings for Corrosion Pennysylvinia, pp. 159–170.
Control, ACS Symposium Series, Vol. 689. ACS, Washington, DC,
Pendyala, J., Avci, R., Geesey, G.G., Stoodley, P., Hamilton, M., Harkin,
G., 1996. Chemical e ect of bioÿlm colonization on 304 stainless
Moore, L., Postle, M., 1994. Risk-beneÿt analysis and case study
steel. Journal of Vacuum Science and Technology A14, 1955–1960.
on tributyl tin. International Biodeterioration & Biodegradation 34,
Pierson, D.L., Mishra, S.K., 1992. Microbiological challenges of
space habitation. 43rd Congress of the International Astronautical
Morton, R.L., Yanko, W.A., Graham, D.W., Arnold, R.G., 1991.
Confederation Congress, Washington, DC.
Relationships between metal concentrations and crown corrosion in Los
Pierson, B.K., Parenteau, M.N., 2000. Phototrophs in high iron microbial
Angeles County sewers. Research Journal of Water Pollution Control
mats: microstructure of mats in iron-depositing hot springs. FEMS
Federation 63, 779–798.
Microbiology Ecology 32, 181–196.
Myers, T., 1988. Failing the test: germicides or use dilution methodology?.
Pi˜ ar, G., Saiz-Jimenez, C., Schabereiter-Gurtner, C., Blanco-Varela,
ASM (American Society for Microbiology) News 54, 19–21.
M.T., Lubitz, W., Rolleke, S., 2001. Archael communities in two
Nakajima-Kambe, T., Onuma, F., Kimpara, N., Nakahara, T., 1995.
disparate deteriorated ancient wall paintings: detection, identiÿcation
Isolation and characterization of a bacterium which utilizes polyester
and temporal monitoring by denaturing gradient gel electrophoresis.
polyurethane as a sole carbon and energy source. FEMS Microbiology
FEMS Microbiology Ecology 37, 45–54.
Letters 129, 39–42.
Nakajima-Kambe, T., Onuma, F., Akutsu, Y., Nakahara, T., 1997. Pitt, C.G., 1992. Non-microbial degradation of polyesters: mechanisms
Determination of the polyester polyurethane breakdown products and and modiÿcations. In: Vert, M., Feijen, J., Albertsson, A., Scott,
distribution of the polyurethane degrading enzyme of Comamonas G., Chiellini, E. (Eds.), Biodegradable Polymers and Plastics. Royal
acidovoran Strain TB-35. Journal of Fermentation and Bioengineering Society of Chemistry, Redwood Press, Melksham, Wiltshire, England,
83, 456–460. pp. 7–17.
Nakanishi, K., Marui, M., Yasui, T., 1992. Comparison of xylan and Pometto, III, A.L., Lee, B., Johnson, K.E., 1992. Production of
methyl ÿ-xyloside-induced xylanases from Streptomyces sp. Journal an extracellular polyethylene-degrading enzyme(s) by Streptomyces
of Fermentation and Bioengineering 74, 392–394. species. Applied and Environmental Microbiology 58, 731–733.
Nakayama, K., Saito, T., Fukui, Y., Shirakura, Y., Tomita, K., 1985. Pometto, III, A.L., Johnson, K.E., Kim, M., 1993. Pure-culture
Puriÿcation and properties of extracellular poly(3-hydroxybutyrate) and enzymatic assay for starch-polyethylene degradable plastic
depolymerases from Pseudomonas lemoignei. Biochimica et biodegradation with Streptomyces species. Journal of Environmental
Biophysica Acta 827, 63–72. Polymer Degradation 1, 213–221.
Narayan, R., 1993. Biodegradation of polymeric materials (anthropogenic Power, K., Marshall, K.C., 1988. Cellular growth and reproduction of
macromolecules) during composting. In: Hoitink, H.A.J., Keener, marine bacteria on surface-bound substrate. Biofouling 1, 163–174.
H.M. (Eds.), Science and Engineering of Composting: Design, Pyle, B.H., Broadaway, S.C., McFeters, G.A., 1992. E cacy of copper
Environmental, Microbiological and Utilization Aspects. Renaissance and silver ions with iodine in the inactivation of Pseudomonas cepacia.
Publishers, Washington, OH, pp. 339–362. Journal of Applied Bacteriology 72, 71–79.
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 89
Raychaudhuri, S., Sutphin, P.D., Chang, J.T., Altman, R.B., 2001. Severini, F., Gallo, R., Ipsale, S., 1988. Environmental degradation of
Basic microarray analysis: grouping and feature reduction. Trends in polypropylene. Polymer Degradability and Stability 22, 185–194.
Biotechnology 19, 189–193. Sharp, R.R., Bryers, J.B., Jones, W.G., Shields, M.S., 1998. Activity and
Reese, E.T., 1957. Biological degradation of cellulose derivatives. stability of a recombinant plasmid-borne TCE degradative pathway in
Industrial Engineering and Chemistry 49, 89–93. suspended cultures. Biotechnology and Bioengineering 57, 287–296.
Reinsel, M.A., Sears, J.T., Stewart, P.S., Mclnerney, M.J., 1996. Control Sneath, P.H.A., Mair, N.S., Sharpe, M.E., Holt, J.G., 1986. Bergey’s
of microbial souring by nitrate, nitrite or glutaraldehyde injection in a Manual of Systematic Bacteriology, Vol. 2. Williams and Wilkins,
sandstone column. Journal of Industrial Microbiology 17, 128–136. Baltimore, MD.
Rethke, D., 1994. Testing of Russian ECLSS-Sabatier and potable water Sneider, R.P., Chadwick, B.R., Pembrey, R., Jankowski, J., Acworth,
processor. SAE Technical Paper 941252, Intersociety Conference on I., 1994. Retention of the Gram-negative bacterium SW8 on surfaces
Environmental Systems, Friedrichschafen, Germany. under conditions relevant to the subsurface environment: e ects of
Reynolds, T.B., Fink, G.R., 2001. Baker’s yeast, a model for fungal conditioning ÿlms and substratum nature. FEMS Microbiology Ecology
bioÿlm formation. Science 291, 878–881. 14, 243–254.
Rijnaarts, H.H.M., Norde, W., Bouwer, E.J., Lyklema, J., Zehnder, A.J.B., Solomin, G.I., 1985. Problem of combined toxicological and hygenic
1993. Bacterial adhesion under static and dynamic conditions. Applied evaluation of polymer construction materials. Kosmicheskaya
and Environmental Microbiology 59, 3255–3265. Biologiya i Aviakosmicheskaya Medistina 19, 4–11 (in Russian).
Rittman, B.E., 1993. The signiÿcance of bioÿlms in porous media. Water Sonne-Hansen, J., Mathrani, I.M., Ahring, B.K., 1993. Xylanolytic
Resource Research 29, 2195–2202. anaerobic thermophiles from icelandic hot-springs. Applied
Rogers, J., Dowsett, A.B., Dennis, P.J., Lee, J.V., Keevil, C.W., 1994. Microbiology and Biotechnology 38, 537–541.
In uence of pluming materials on bioÿlm formation and growth Srinivasan, R., Stewart, P.S., Griebe, T., Chen, C.-I., 1995.
of Legionella pneumophila in potable water systems. Applied and Bioÿlm parameters in uencing biocide e cacy. Biotechnology and
Environmental Microbiology 60, 1842–1851. Bioengineering 46, 553–560.
Rolleke, S., Witte, A., Wanner, G., Lubitz, W., 1998. Medieval wall Staley, J.T., Bryant, M.P., Pfenning, N., Holt, J.G., 1989. Bergey’s Manual
paintings—a habitat for archaea: identiÿcation of archaea by denaturing of Systematic Bacteriology, Vol. 3. Williams and Wilkins, Baltimore,
gradient gel electrophoresis (DGGE) of PCR-ampliÿed gene fragments MD.
coding for 16S rRNA in a medieval wall painting. International Stenbuchel, A., 1991. Polyhydroxyalkanoic acids. In: Byrom, D. (Ed.),
Biodeterioration & Biodegradation 41, 85–92. Biomaterials: Novel Materials from Biological Sources. Macmillan,
Rossmoore, H.W., Rossmoore, L.A., 1993. MIC in metalworking New York, pp. 127–213.
processes and hydraulic systems. In: Kobrin, G. (Ed.), A Stern, R.V., Howard, G.T., 2000. The polyester polyurethanase gene
Practical Manual on Microbiologically In uenced Corrosion. NACE (pue A) from Pseudomonas chlororaphis encodes a lipase. FEMS
International, Houston, Texas, pp. 31–40. Microbiology Letters 185, 163–168.
Saiz-Jimenez, C., 1995. Deposition of anthropogenic compounds on Sternberg, D., Vigayakumar, P., Reese, E.T., 1977. ÿ-Glucosidase:
monuments and their e ect on airborne microorganisms. Aerobiologia microbial production and e ect on enzymatic hydrolysis of cellulose.
11, 161–175. Canadian Journal of Microbiology 23, 139–147.
Saiz-Jimenez, C., 1997. Biodeterioration vs. biodegradation: the role Stewart, P.S., 1996. Theoretical aspects of antibiotic di usion into
of microorganisms in the removal of pollutants deposited on microbial bioÿlms. Antimicrobial Agents and Chemotheraphy 40,
historic buildings. International Biodeterioration & Biodegradation 40, 2517–2522.
225–232. Stewart, P.S., Hamilton, M.A., Goldstein, B.R., Schneider, B.T.,
Saito, T., Suzuki, Yamamoto, K., Fukui, T., Miwa, K., Tomita, K., 1996. Modeling biocide action against bioÿlms. Biotechnology and
Nakanishi, S., Odani, S., Suzuki, J.-I., Ishikawa, K., 1989. Cloning, Bioengineering 49, 445–455.
nucleotide sequence, and expression in Escherichia coli of the gene Stoodley, P., DeBeer, D., Lappin-Scott, H.M., 1997. In uence of electric
for poly-3-hydroxybutyrate depolymerase from Alcaligenes faecalis. ÿelds and pH on bioÿlm structure as related to the bioelectric e ect.
Journal of Bacteriology 171, 184 –189. Antmicrobial Agents and Chemotheraphy 41, 1876–1879.
Salama, N., Guillemin, K., McDaniel, T.K., Sherlock, G., Tompkins, L., Stranger-Joannesen, M.R., Sorheim, D., Zanotti, Bichi, A., 1993.
Falkow, S., 2000. A whole-genome microarray reveals genetic diversity The ESA-LPTO simulation campaigns: microbial contamination
among Helicobacter pylori strains. Proceedings of National Academy of the closed manned habitats. Proceedings of the 44th
of Science (USA) 97, 14668–14673. Congress of the International Astronautical Confederation Congress,
Salmond, G.P.C., Bycroft, B.W., Stewart, G.S.A.B., Williams, P., 1995. IAF/IAA-93-G.4.162, Graz, Austria.
The bacterial ‘enigma’: cracking the code of cell–cell communication. Stuart, E.S., Lenz, R.W., Fuller, R.C., 1995. The ordered macromolecular
Molecular Microbiology 16, 615–624. surface of polyester inclusion bodies in Pseudomonas oleovorans.
Sand, W., Ahlers, B., Bock, E., 1991. The impact of microorganisms— Canadian Journal of Microbiology 41 (Suppl.), 84–93.
especially nitric acid producing bacteria—on the deterioration of Suci, P.A., Vrany, J.D., Mittelamn, M.W., 1998. Investigation of
natural stones. In: Baer, N.S., Sabbioni, C., Sors, A.I. (Eds.), Science, interactions between antimicrobial agents and bacterial bioÿlms using
Technology and European Cultural Heritage. Butterworth-Heinemann, attenuated total re ection Fourier transform infrared spectroscopy.
Oxford, England, pp. 481–484. Biomaterials 19, 327–339.
Scamans, G.M., Hunter, J.A., Holroyd, N.J.H., 1989. A Sullivan, B.K., Oviatt, C.A., Klein-MacPhee, G., 1993. Fate and
surface-engineering approach to the corrosion aluminum. Treatise on e ects of a starch-based biodegradable plastic substitute in the
Materials Science and Technology 31, 485–500. marine environment. In: Kaplan, D., Thomas, E., Ching, C. (Eds.),
Schink, B., Stieb, M., 1983. Fermentative degradation of polyethylene Fundamentals of Biodegradable Materials and Packaging. Technomic
glycol by a strictly anaerobic, Gram-negative, non-spore-forming Publishing Co, Lancaster, Pennsylvania, pp. 281–296.
bacterium, Pelobacter venetianus sp. nov. Applied and Environmental Sunesson, A., Vaes, W.H.J., Nilsson, C., Blomouist, G., Andersson, B.,
Microbiology 45, 1905–1913. Carlson, R., 1995. Identiÿcation of volatile metabolites from ÿve
Schmidt, R., 1997. Monte Carlo simulation of bioadhesion. International fungal species cultivated on two media. Applied and Environmental
Biodeterioration & Biodegradation 40, 29–36. Microbiology 61, 2911–2918.
Selwitz, C.M., 1992. The use of epoxy resins in ÿeld projects for stone Swift, M.J., Heal, O.W., Anderson, J.M., 1979. Decomposition in
stabilization. Materials Research Society Symposium Proceedings 267, terrestrial ecosystems. In: Studies in Ecology, Vol. 5. Blackwell,
925–934. Great Britain.
90 J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91
Szycher, M., 1989. Medical-grade polyurethanes: their crucial role Wagner, P., 1995. Microbial degradation of stressed ÿber reinforced
in artiÿcial hearts. In: Materials Research Society Symposium polymeric composites. Corrosion/95, Paper No. 200, NACE
Proceedings, Vol. 110. Materials Research Society, Pittsburgh, International, Houston, Texas.
Pennsylvania, pp. 41–50. Wagner, P., Ray, R., Hart, K., Little, B., 1996. Microbiological
Tall, B.D., Williams, H.N., George, K.S., Gray, R.T., Walch, M., 1995. degradation of stressed ÿber-reinforced polymeric composites.
Bacterial succession within a bioÿlm in water supply lines of dental Materials Perfomance 35, 79–82.
air–water syringes. Canadian Journal of Microbiology 41, 647–654. Wakeÿeld, R.D., 1997. Masonary biocides-assessments of e cacy and
Tanio, T., Fukui, T., Saito, T., Tomita, K., Kaiho, T., Masamune, S., e ects on stone. Scotish Society of Conservation Restaurators 8, 5–11.
1982. An extracellular poly(ÿ-hydroxybutyrate) depolymerase from Walch, M., 1992. Corrosion, microbial. Encyclopedia of Microbiology 1,
Alcaligenes faecalis. European Journal of Biochemistry 124, 71–77. 585–591.
Thorp, K.E.G., Crasto, A.S., Gu, J.-D., Mitchell, R., 1994. Biodegradation Wang, C.-C., Fan, C.-Z., Wang, S.-J., Zhang, M.-G., 1991. Research on
of composite materials. In: Naguy, T. (Ed.), Proceedings of the powdery corrosion of the Serials Bells from Cai Hou Tomb. Science
Tri-Service Conference on Corrosion. U.S. Government Printing China (Series B) 34, 522–529.
House, Washington, DC, pp. 303–314. Wang, C.-C., Wu, Y.-S., Fan, C.-Z., Wang, S.-J., Hua, Y.-M., 1993.
Formation mechanism of particulates in the surface layer of Bronze
Thorp, K.E.G., Crasto, A.S., Gu, J.-D., Mitchell, R., 1997. Contribution
Mirror. China Science Bulletin 38, 429–432.
of microorganisms to corrosion. Corrosion/97, Paper No. 279, National
Wang, Y., Fan, Y., Gu, J.-D., 2003. Degradation of phthalic acid and
Association of Corrosion Engineers, Houston, Texas.
dimethyl phthalate by aerobic microorganisms. Chinese Journal of
Tilstra, L., Johnsonbaugh, D., 1993. A test method to determine rapidly
Applied and Environmental Biology, in press.
if polymers are biodegradable. Journal of Environmental Polymer
Whitÿeld, C., 1988. Bacterial extracellular polysaccharides. Canadian
Degradation 1, 247–255.
Journal of Microbiology 34, 415–420.
Torronen, A., Kubicek, C.P., Henrissat, B., 1993. Amino acid sequence Wiencek, K.M., Fletcher, M., 1995. Bacterial adhesion to hydroxyl- and
similarities between low molecular weight endo-1,4-ÿ-xylanases and methyl-terminated alkanethiol self-assembled monolayers. Journal of
family H cellulases revealed by clustering analysis. FEBS Letters 321, Bacteriology 177, 1959–1966.
135–139. Wilkinson, J.F., Stark, G.H., 1956. The synthesis of polysaccharide by
Tsao, R., Anderson, T.A., Coats, J.R., 1993. The in uence of soil washed suspensions of Klebsiella aerogenes. Proceedings of Royal
macroinvertebrates on primary biodegradation of starch-containing Physics Society Edinburgh 25, 35–39.
polyethylene ÿlms. Journal of Environmental Polymer Degradation 1, Williams, V., Fletcher, M., 1996. Pseudomonas uorescens adhesion
301–306. and transport through porous media are a ected by lipopolysaccharide
van Loosdrecht, M.C.M., Lyklema, J., Norde, W., Schraa, G., Zehnder, composition. Applied and Environmental Microbiology 62, 100–104.
A.J.B., 1987. The role of bacterial cell wall hydrophobicity in adhesion. Williams, S.T., Sharpe, M.E., Holt, J.G., 1989. Bergey’s Manual of
Applied and Environmental Microbiology 53, 1893–1897. Systematic Bacteriology, Vol. 4. Williams and Wilkins, Baltimore,
van Loosdrecht, M.C.M., Lyklema, J., Norde, W., Schraa, G., MD.
Zehnder, A.J.B., 1990. In uence of interfaces on microbial activity. Williamson, P.R., 1994. The screening of sponge extracts for antifouling
Microbiological Review 54, 75–87. activity using a bioassay with laboratory-reared cyprid larvae of
Vandevivere, P., 1995. Bacterial clogging of porous media: a new the barnacle Balanus amphitrite. International Biodeterioration &
modelling approach. Bifouling 8, 281–291. Biodegradation 34, 361–373.
Vandevivere, P., Kirchman, D.L., 1993. Attachment stimulates Wimpenny, J.W.T., Colasanti, R., 1997. A unifying hypothesis for the
exopolysaccharide synthesis by a bacterium. Applied and structure of microbial bioÿlm based on cellular automaton models.
Environmental Microbiology 59, 3280–3286. FEMS Microbiology Ecology 22, 1–6.
van Westing, E.P.M., Ferrari, G.M., De Witt, J.H.W., 1994. The Wirsen, C.O., Jannasch, H.W., 1993. Microbial degradation of a
determination of coating performance with impedance measurements. starch-based biopolymer in the marine environment. In: Kaplan,
II. Water uptake of coatings. Corrosion Science 36, 957–977. D., Thomas, E., Ching, C. (Eds.), Fundamentals of Biodegradable
Verbicky, J.W., 1988. Polyimides. In: Encyclopedia of Polymer Science Materials and Packaging. Technomic Publishing Co, Lancaster,
and Engineering, Vol. 12. Wiley, New York, pp. 364 –383. Pennsylvania, pp. 297–310.
Verbiest, T., Burland, D.M., Jurich, M.C., Lee, V.Y., Miller, R.D., Woese, C.R., 1987. Microbial Evolution. Microbiological Review 51,
Volksen, W., 1995. Exceptionally thermally stable polyimides for 221–271.
Wolfaardt, G.M., Lawrence, J.R., Robarts, R.D., Caldwell, S.J., Caldwell,
second-order nonlinear optical applications. Science 268, 1604–1606.
D.E., 1994. Multicellular organization in a degradative bioÿlm
Viktorov, A.N., 1994. The characteristics of interaction between normal
community. Applied and Environmental Microbiology 60, 434–446.
and conventionally pathogenic human micro ora in di erent types of
Wong, K.K.Y., Tan, L.U.L., Saddler, J.N., 1988. Multiplicity
closed objects. Proceedings of the 45th Congress of the International
of ÿ-1,4-xylanase in microorganisms: function and applications.
Astronautical Confederation Congress, IAF/IAA-94-5.165, Jerusalem,
Microbiological Review 52, 305–317.
Wu, Y.-S., Wang, C.-S., Fan, C.-Z., Wang, S.-J., Li, Z.-C., 1992. A study
Viktorov, A.N., Novikova, N.D., 1985. Distinctions in formation of
on corrosion-resistance mechanism of the ancient mirror “Hei Qi Gu”.
micro ora on construction materials used in habitable pressurized
Acta Physica Sinica 41, 170–176.
compartments. Kosmicheskaya Biologiya i Aviakosmicheskaya Xu, X., Stewart, P.S., Chen, X., 1996. Transport limitation of chlorine
Medistina 19, 66–69 (in Russian). disinfection of Pseudomonas aeruginosa entrapped in alginate beads.
Viktorov, A.N., IIyin, V.K., 1992. The actual problems of microbiological Biotechnology and Bioengineering 49, 93–100.
control in regenerative life support systems exploration. Proceedings Yoshizako, F., Nishimura, A., Chubachi, M., 1992. Microbial reduction
of the 43rd Congress of the International Astronautical Confederation of cyclohexanone by Chlorella pyrenoidosa chick. Journal of
Congress, IAF/IAA-92-0277, Washington, DC. Fermentation and Bioengineering 74, 395–397.
Viktorov, A.N., IIyin, V.K., Syniak, J., 1993. The problems of microbial You, Z., Fukushima, J., Tanka, K., Kawamoto, S., Okuda, K., 1998.
safety in regenerative life support systems exploration. Proceedings Induction of entry into the stationary growth phase in Pseudomonas
of the 44th Congress of the International Astronautical Confederation aeruginosa by N -acylhomoserine lactone. FEMS Microbiology Letters
Congress, IAF/IAA-93-G.4.161, Graza, Austria. 164, 99–106.
Wachtershauser, G., 1988. Before enzymes and templates: theory of Young, G.H., 1948. Anti-fouling measures. In: Uhlig, H.H. (Ed.), The
surface metabolism. Microbiological Review 52, 452–484. Corrosion Handbook. Wiley, New York, pp. 441–446.
J.-D. Gu / International Biodeterioration & Biodegradation 52 (2003) 69 – 91 91
Yu, F.P., McFeters, G.A., 1994. Physiological responses of bacteria in Zehnder, A.J.B., Stumm, W., 1988. Geochemistry and biochemistry of
bioÿlms to disinfection. Applied and Environmental Microbiology 60, anaerobic habitats. In: Zehnder, A.J.B. (Ed.), Biology of Anaerobic
2462–2466. Microorganisms. Wiley, New York, pp. 1–38.
Zachary, A., Taylor, M.E., Scott, F.E., Colwell, R.R., 1980. Marine Zhou, Z., Brown, N., 1995. Slow crack growth in polyethylene gas pipes
microbial colonization on material surfaces. In: Oxley, T.A., Becker, and resins. Chinese Journal of Materials Research 9 (Suppl.), 463–472.
G., Allsopp, D. (Eds.), Biodeterioration: Proceedings of the fourth Zou, J., Xu, C., Liu, X., Wang, C., 1994. Study of the Raman spectrum
International Biodeterioration Symposium. Pitman Publishing Ltd, of nanometer SnO2 . Journal of Applied Physics 75, 1835–1836.
London, pp. 171–177. Zyska, B., 1996. Performance of paper in Polish books of the period
Zaloguyev, S.N., 1985. Results of microbiological studies conducted 1900 –1994. Restaurator 17, 214–228.
during operation of Slyut-6 orbital space station. Kosmicheskaya
Biologiya i Aviakosmicheskaya Medistina 19, 64–66 (in Russian).